View stunning SlideShares in full-screen with the new iOS app!Introducing SlideShare for AndroidExplore all your favorite topics in the SlideShare appGet the SlideShare app to Save for Later — even offline
View stunning SlideShares in full-screen with the new Android app!View stunning SlideShares in full-screen with the new iOS app!
Mechanical Engineers’ Handbook
JOHN WILEY & SONS, INC.
This book is printed on acid-free paper. ࠗϱ
Copyright ᭧ 2006 by John Wiley & Sons, Inc. All rights reserved.
Published by John Wiley & Sons, Inc., Hoboken, New Jersey.
Published simultaneously in Canada.
No part of this publication may be reproduced, stored in a retrieval system, or transmitted in any form
or by any means, electronic, mechanical, photocopying, recording, scanning, or otherwise, except as
permitted under Section 107 or 108 of the 1976 United States Copyright Act, without either the prior
written permission of the Publisher, or authorization through payment of the appropriate per-copy fee
to the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, (978) 750-8400,
fax (978) 750-4470, or on the web at www.copyright.com. Requests to the Publisher for permission
should be addressed to the Permissions Department, John Wiley & Sons, Inc., 111 River Street,
Hoboken, NJ 07030, (201) 748-6011, fax (201) 748-6008, or online at http://www.wiley.com/go/
Limit of Liability/Disclaimer of Warranty: While the publisher and author have used their best efforts
in preparing this book, they make no representations or warranties with respect to the accuracy or
completeness of the contents of this book and speciﬁcally disclaim any implied warranties of
merchantability or ﬁtness for a particular purpose. No warranty may be created or extended by sales
representatives or written sales materials. The advice and strategies contained herein may not be
suitable for your situation. The publisher is not engaged in rendering professional services, and you
should consult a professional where appropriate. Neither the publisher nor author shall be liable for
any loss of proﬁt or any other commercial damages, including but not limited to special, incidental,
consequential, or other damages.
For general information on our other products and services, please contact our Customer Care
Department within the United States at (800) 762-2974, outside the United States at (317) 572-3993
or fax (317) 572-4002.
Wiley also publishes its books in a variety of electronic formats. Some content that appears in print
may not be available in electronic books. For more information about Wiley products, visit our web
site at www.wiley.com.
Library of Congress Cataloging-in-Publication Data:
Mechanical engineers’ handbook/edited by Myer Kutz.—3rd ed.
Includes bibliographical references and index.
ISBN-10 0-471-44990-3 (cloth)
1. Mechanical engineering—Handbooks, manuals, etc. I. Kutz, Myer.
Printed in the United States of America.
10 9 8 7 6 5 4 3 2 1
Vision Statement xi
PART 1 MATERIALS 1
1. Carbon and Alloy Steels 3
Bruce L. Bramﬁtt
2. Stainless Steels 39
3. Aluminum Alloys 59
J. G. Kaufman
4. Copper and Copper Alloys 117
Konrad J. A. Kundig and John G. Cowie
5. Selection of Titanium Alloys for Design 221
Matthew J. Donachie
6. Nickel and Its Alloys 256
Gaylord D. Smith and Brian A. Baker
7. Magnesium and Its Alloys 278
Robert E. Brown
8. Selection of Superalloys for Design 287
Matthew J. Donachie and Stephen J. Donachie
9. Plastics: Information and Properties of Polymeric Materials 335
Edward N. Peters
10. Composite Materials 380
11. Smart Materials 418
James A. Harvey
12. Overview of Ceramic Materials, Design, and Application 433
R. Nathan Katz
13. Sources of Materials Data 450
J. G. Kaufman
14. Quantitative Methods of Materials Selection 466
Mahmoud M. Farag
PART 2 MECHANICAL DESIGN 489
15. Stress Analysis 491
Franklin E. Fisher
16. An Introduction to the Finite-Element Method 557
Tarek I. Zohdi
17. Design for Six Sigma: A Mandate for Competitiveness 581
James E. McMunigal and H. Barry Bebb
18. TRIZ 612
James E. McMunigal, Steven Ungvari, Michael Slocum, and Ruth E. McMunigal
19. Computer-Aided Design 642
Emory W. Zimmers, Jr., and Technical Staff of Enterprise Systems Center
20. Data Exchange Using STEP 725
21. Engineering Applications of Virtual Reality 732
Xiaobo Peng and Ming C. Leu
Maury A. Nussbaum and Jaap H. van Diee¨n
23. Electronic Materials and Packaging 782
Warren C. Fackler
24. Design Optimization: An Overview 819
A. Ravi Ravindran and G. V. Reklaitis
25. Design for Manufacturing and Assembly with Plastics 847
James A. Harvey
26. Failure Modes: Performance and Service Requirements for Metals 860
J. A. Collins and S. R. Daniewicz
27. Failure Analysis of Plastics 925
Vishu H. Shah
28. Failure Modes: Performance and Service Requirements for Ceramics 942
29. Mechanical Reliability and Life Prediction for Brittle Materials 962
G. S. White, E. R. Fuller, Jr., and S. W. Freiman
30. Total Quality Management in Mechanical Design 980
B. S. Dhillon
31. Reliability in the Mechanical Design Process 1000
B. S. Dhillon
32. Lubrication of Machine Elements 1024
Bernard J. Hamrock
33. Seal Technology 1161
Bruce M. Steinetz
34. Vibration and Shock 1204
Singiresu S. Rao
35. Noise Measurement and Control 1230
George M. Diehl
36. Nondestructive Inspection 1253
Robert L. Crane and Jeremy S. Knopp
The ﬁrst volume of the third edition of the Mechanical Engineers’ Handbook is comprised
of two major parts. The ﬁrst part, Materials, which has 14 chapters, covers metals, plastics,
composites, ceramics, and smart materials. The metals covered are carbon, alloy, and stain-
less steels; aluminum and aluminum alloys; copper and copper alloys; titanium alloys; nickel
and its alloys; magnesium and its alloys; and superalloys. Chapters on some of these ma-
terials, such as ceramics, smart materials, and superalloys, are updated versions of chapters
that have appeared in the Handbook of Materials Selection (Wiley, 2002), and they are
entirely new to the Mechanical Engineers’ Handbook. The intent in all of the materials
chapters is to provide readers with expert advice on how particular materials are typically
used and what criteria make them suitable for speciﬁc purposes. This part of Volume I
concludes with a chapter on sources of materials data, the intent being to provide readers
with guidance on ﬁnding reliable information on materials properties, in addition to those
that can be found in this volume, and a chapter on analytical methods of materials selection,
which is intended to give readers techniques for specifying which materials might be suitable
for a particular application.
The second part of Volume I, Mechanical Design, which has 22 chapters, covers a broad
range of topics, including the fundamentals of stress analysis, the ﬁnite-element method,
vibration and shock, and noise measurement and control and then moving into modern
methodologies that engineers use to predict failures, eliminate defects, enhance quality and
reliability of designs, and optimize designs. There are chapters on failure analysis and design
with all classes of materials, including metals, plastics and ceramics, and composites. I should
point out that, to a large extent, the two parts of Volume I go hand in hand. After all, it is
useful to know about the properties, behavior, and failure mechanisms of all classes of
materials when faced with a product design problem. Coverage in the second part of Volume
I extends to lubrication of machine elements and seals technology. Chapters in this part of
Volume I provide practitioners with techniques to solve real, practical everyday problems,
ranging from nondestructive testing to CAD (computer-aided design) to TRIZ (the acronym
in Russian for Theory of Inventive Problem Solving), STEP [the Standard for the Exchange
of Product Model Data is a comprehensive International Organization for Standardization
standard (ISO 10303) that describes how to represent and exchange digital product infor-
mation], and virtual reality. Topics of special interest include physical ergonomics and elec-
While many of the chapters in Volume I are updates or entirely new versions of chapters
from the second edition of the Mechanical Engineers’ Handbook and the Handbook of
Materials Selection, a number of chapters—on Six Sigma, TRIZ, and STEP—are new ad-
ditions to this family of handbooks. Contributors of the chapters in Volume I include pro-
fessors, engineers working in industry and government installations, and consultants, mainly
from North America, but also from Egypt, the Netherlands, and Germany.
Vision for the Third Edition
Basic engineering disciplines are not static, no matter how old and well established they are.
The ﬁeld of mechanical engineering is no exception. Movement within this broadly based
discipline is multidimensional. Even the classic subjects on which the discipline was founded,
such as mechanics of materials and heat transfer, continue to evolve. Mechanical engineers
continue to be heavily involved with disciplines allied to mechanical engineering, such as
industrial and manufacturing engineering, which are also constantly evolving. Advances in
other major disciplines, such as electrical and electronics engineering, have signiﬁcant impact
on the work of mechanical engineers. New subject areas, such as neural networks, suddenly
become all the rage.
In response to this exciting, dynamic atmosphere, the Mechanical Engineers’Handbook
is expanding dramatically, from one volume to four volumes. The third edition not only is
incorporating updates and revisions to chapters in the second edition, which was published
in 1998, but also is adding 24 chapters on entirely new subjects as well, incorporating updates
and revisions to chapters in the Handbook of Materials Selection, which was published in
2002, as well as to chapters in Instrumentation and Control, edited by Chester Nachtigal
and published in 1990.
The four volumes of the third edition are arranged as follows:
Volume I: Materials and Mechanical Design—36 chapters
Part 1. Materials—14 chapters
Part 2. Mechanical Design—22 chapters
Volume II: Instrumentation, Systems, Controls, and MEMS—21 chapters
Part 1. Instrumentation—8 chapters
Part 2. Systems, Controls, and MEMS—13 chapters
Volume III: Manufacturing and Management—24 chapters
Part 1. Manufacturing—12 chapters
Part 2. Management, Finance, Quality, Law, and Research—12 chapters
Volume IV: Energy and Power—31 chapters
Part 1: Energy—15 chapters
Part 2: Power—16 chapters
The mechanical engineering literature is extensive and has been so for a considerable
period of time. Many textbooks, reference works, and manuals as well as a substantial
number of journals exist. Numerous commercial publishers and professional societies, par-
ticularly in the United States and Europe, distribute these materials. The literature grows
continuously, as applied mechanical engineering research ﬁnds new ways of designing, con-
trolling, measuring, making and maintaining things, and monitoring and evaluating technol-
ogies, infrastructures, and systems.
Most professional-level mechanical engineering publications tend to be specialized, di-
rected to the speciﬁc needs of particular groups of practitioners. Overall, however, the me-
chanical engineering audience is broad and multidisciplinary. Practitioners work in a variety
of organizations, including institutions of higher learning, design, manufacturing, and con-
xii Vision for the Third Edition
sulting ﬁrms as well as federal, state, and local government agencies. A rationale for an
expanded general mechanical engineering handbook is that every practitioner, researcher,
and bureaucrat cannot be an expert on every topic, especially in so broad and multidiscipli-
nary a ﬁeld, and may need an authoritative professional summary of a subject with which
he or she is not intimately familiar.
Starting with the ﬁrst edition, which was published in 1986, our intention has always
been that the Mechanical Engineers’ Handbook stand at the intersection of textbooks, re-
search papers, and design manuals. For example, we want the handbook to help young
engineers move from the college classroom to the professional ofﬁce and laboratory where
they may have to deal with issues and problems in areas they have not studied extensively
With this expanded third edition, we have produced a practical reference for the me-
chanical engineer who is seeking to answer a question, solve a problem, reduce a cost, or
improve a system or facility. The handbook is not a research monograph. The chapters offer
design techniques, illustrate successful applications, or provide guidelines to improving the
performance, the life expectancy, the effectiveness, or the usefulness of parts, assemblies,
and systems. The purpose is to show readers what options are available in a particular
situation and which option they might choose to solve problems at hand.
The aim of this expanded handbook is to serve as a source of practical advice to readers.
We hope that the handbook will be the ﬁrst information resource a practicing engineer
consults when faced with a new problem or opportunity—even before turning to other print
sources, even ofﬁcially sanctioned ones, or to sites on the Internet. (The second edition has
been available online on knovel.com.) In each chapter, the reader should feel that he or she
is in the hands of an experienced consultant who is providing sensible advice that can lead
to beneﬁcial action and results.
Can a single handbook, even spread out over four volumes, cover this broad, interdis-
ciplinary ﬁeld? We have designed the third edition of the Mechanical Engineers’Handbook
as if it were serving as a core for an Internet-based information source. Many chapters in
the handbook point readers to information sources on the Web dealing with the subjects
addressed. Furthermore, where appropriate, enough analytical techniques and data are pro-
vided to allow the reader to employ a preliminary approach to solving problems.
The contributors have written, to the extent their backgrounds and capabilities make
possible, in a style that reﬂects practical discussion informed by real-world experience. We
would like readers to feel that they are in the presence of experienced teachers and con-
sultants who know about the multiplicity of technical issues that impinge on any topic within
mechanical engineering. At the same time, the level is such that students and recent graduates
can ﬁnd the handbook as accessible as experienced engineers.
Brian A. Baker
Special Metals Corporation
Huntington, West Virginia
H. Barry Bebb
San Diego, California
Bruce L. Bramﬁtt
International Steel Group, Inc.
Robert E. Brown
Magnesium Monthly Review
J. A. Collins
The Ohio State University
John G. Cowie
Copper Development Association
New York, New York
Robert L. Crane
Wright Patterson Air Force Base
S. R. Daniewicz
Mississippi State University
B. S. Dhillon
University of Ottawa
Ottawa, Ontario, Canada
Jaap H. van Diee¨n
Amsterdam, The Netherlands
George M. Diehl
Phillipsburg, New Jersey
Matthew J. Donachie
Rennselaer at Hartford
Stephen J. Donachie
Special Metals Corporation
Huntington, West Virginia
Warren C. Fackler
Cedar Rapids, Iowa
Mahmoud M. Farag
The American University in Cairo
Franklin E. Fisher
Loyola Marymount University
Los Angeles, Calaifornia
El Segundo, California
S. W. Freiman
National Institute of Standards and
E. R. Fuller, Jr.
National Institute of Standards and
Bernard J. Hamrock
The Ohio State University
STEP Tools, Inc.
Troy, New York
James A. Harvey
Under the Bridge Consulting, Inc.
R. Nathan Katz
Worcester Polytechnic Institute
J. G. Kaufman
Jeremy S. Knopp
Wright Patterson Air Force Base
Konrad J. A. Kundig
Ming C. Leu
University of Missouri-Rolla
James E. McMunigal
Long Beach, California
Ruth E. McMunigal
Long Beach, California
University of Karlsruhe
Maury A. Nussbaum
Virginia Polytechnic Institute and State
University of Missouri-Rolla
Edward N. Peters
General Electric Company
Selkirk, New York
Singiresu S. Rao
University of Miami
Coral Gables, Florida
A. Ravi Ravindran
Pennsylvania State University
University Park, Pennsylvania
G. V. Reklaitis
West Lafayette, Indiana
Breakthrough Management Group
Vishu H. Shah
Gaylord D. Smith
Special Metals Corporation
Huntington, West Virginia
Bruce M. Steinetz
NASA Glenn Research Center at Lewis
Strategic Product Innovations, Inc.
G. S. White
National Institute of Standards and
Emory W. Zimmers, Jr..
Tarek I. Zohdi
University of California
CARBON AND ALLOY STEELS
Bruce L. Bramﬁtt
International Steel Group, Inc.
1 INTRODUCTION 3
2 STEEL MANUFACTURE 4
3 DEVELOPMENT OF STEEL
4 ROLE OF ALLOYING
ELEMENTS IN STEEL 18
5 HEAT TREATMENT OF STEEL 25
6 CLASSIFICATION AND
SPECIFICATIONS OF STEELS 26
6.1 Carbon Steels 27
6.2 Alloy Steels 29
7 SUMMARY 37
Steel is the most common and widely used metallic material in today’s society. It can be
cast or wrought into numerous forms and can be produced with tensile strengths exceeding
5 GPa. A prime example of the versatility of steel is in the automobile where it is the
material of choice and accounts for over 60% of the weight of the vehicle. Steel is highly
formable as seen in the contours of the automobile outerbody. Steel is strong and is used in
the body frame, motor brackets, driveshaft, and door impact beams of the vehicle. Steel is
corrosion resistant when coated with the various zinc-based coatings available today. Steel
is dent resistant when compared with other materials and provides exceptional energy ab-
sorption in a vehicle collision. Steel is recycled and easily separated from other materials
by a magnet. Steel is inexpensive compared with other competing materials such as alumi-
num and various polymeric materials.
In the past, steel has been described as an alloy of iron and carbon. Today, this descrip-
tion is no longer applicable since in some very important steels, e.g., interstitial-free (IF)
steels and type 409 ferritic stainless steels, carbon is considered an impurity and is present
in quantities of only a few parts per million. By deﬁnition, steel must be at least 50% iron
and must contain one or more alloying elements. These elements generally include carbon,
manganese, silicon, nickel, chromium, molybdenum, vanadium, titanium, niobium, and alu-
minum. Each chemical element has a speciﬁc role to play in the steelmaking process or in
achieving particular properties or characteristics, e.g., strength, hardness, corrosion resistance,
magnetic permeability, and machinability.
Reprinted from Handbook of Materials Selection, Wiley, New York, 2002, by permission of the publisher.
Mechanical Engineers’ Handbook: Materials and Mechanical Design, Volume 1, Third Edition.
Edited by Myer Kutz
Copyright 2006 by John Wiley & Sons, Inc.
4 Carbon and Alloy Steels
2 STEEL MANUFACTURE
In most of the world, steel is manufactured by integrated steel facilities that produce steel
from basic raw materials, i.e., iron ore, coke, and limestone. However, the fastest growing
segment of the steel industry is the ‘‘minimill’’ that melts steel scrap as the raw material.
Both types of facilities produce a wide variety of steel forms, including sheet, plate, struc-
tural, railroad rail, and bar products.
Ironmaking. When making steel from iron ore, a blast furnace chemically reduces the ore
(iron oxide) with carbon in the form of coke. Coke is a spongelike carbon mass that is
produced from coal by heating the coal to expel the organic matter and gasses. Limestone
(calcium carbonate) is added as a ﬂux for easier melting and slag formation. The slag, which
ﬂoats atop the molten iron, absorbs many of the unwanted impurities. The blast furnace is
essentially a tall hollow cylindrical structure with a steel outer shell lined on the inside with
special refractory and graphite brick. The crushed or pelletized ore, coke, and limestone are
added as layers through an opening at the top of the furnace, and chemical reduction takes
place with the aid of a blast of preheated air entering near the bottom of the furnace (an
area called the bosh). The air is blown into the furnace through a number of water-cooled
copper nozzles called tuyeres. The reduced liquid iron ﬁlls the bottom of the furnace and is
tapped from the furnace at speciﬁed intervals of time. The product of the furnace is called
pig iron because in the early days the molten iron was drawn from the furnace and cast
directly into branched mold conﬁgurations on the cast house ﬂoor. The central branch of
iron leading from the furnace was called the ‘‘sow’’ and the side branches were called ‘‘pigs.’’
Today the vast majority of pig iron is poured directly from the furnace into a refractory-
lined vessel (submarine car) and transported in liquid form to a basic oxygen furnace (BOF)
for reﬁnement into steel.
Steelmaking. In the BOF, liquid pig iron comprises the main charge. Steel scrap is added to
dilute the carbon and other impurities in the pig iron. Oxygen gas is blown into the vessel
by means of a top lance submerged below the liquid surface. The oxygen interacts with the
molten pig iron to oxidize undesirable elements. These elements include excess carbon (be-
cause of the coke used in the blast furnace, pig iron contains over 2% carbon), manganese,
and silicon from the ore and limestone and other impurities like sulfur and phosphorus.
While in the BOF, the liquid metal is chemically analyzed to determine the level of carbon
and impurity removal. When ready, the BOF is tilted and the liquid steel is poured into a
refractory-lined ladle. While in the ladle, certain alloying elements can be added to the steel
to produce the desired chemical composition. This process takes place in a ladle treatment
station or ladle furnace where the steel is maintained at a particular temperature by external
heat from electrodes in the lid placed on the ladle. After the desired chemical composition
is achieved, the ladle can be placed in a vacuum chamber to remove undesirable gases such
as hydrogen and oxygen. This process is called degassing and is used for higher quality steel
products such as railroad rail, sheet, plate, bar, and forged products. Stainless steel grades
are usually produced in an induction or electric arc furnace, sometimes under vacuum. To
reﬁne stainless steel, the argon–oxygen decarburization (AOD) process is used. In the AOD,
an argon–oxygen gas mixture is injected through the molten steel to remove carbon without
a substantial loss of chromium (the main element in stainless steel).
Continuous Casting. Today, most steel is cast into solid form in acontinuous-casting (also
called strand casting) machine. Here, the liquid begins solidiﬁcation in a water-cooled copper
mold while the steel billet, slab, or bloom is withdrawn from the bottom of the mold. The
3 Development of Steel Properties 5
partially solidiﬁed shape is continuously withdrawn from the machine and cut to length for
further processing. The continuous-casting process can proceed for days or weeks as ladle
after ladle of molten steel feeds the casting machine. Some steels are not continuously cast
but are poured into individual cast-iron molds to form an ingot that is later reduced in size
by forging or a rolling process to some other shape. Since the continuous-casting process
offers substantial economic and quality advantages over ingot casting, most steel in the world
is produced by continuous casting.
Rolling/Forging. Once cast into billet, slab, or bloom form, the steel is hot rolled through
a series of rolling mills or squeezed/hammered by forging to produce the ﬁnal shape. To
form hot-rolled sheet, a 50–300-mm-thick slab is reduced to ﬁnal thickness, e.g., 2 mm, in
one or more roughing stands followed by a series of six or seven ﬁnishing stands. To obtain
thinner steel sheet, e.g., 0.5 mm, the hot-rolled sheet must be pickled in acid to remove the
iron oxide scale and further cold rolled in a series of rolling stands called a tandem mill.
Because the cold-rolling process produces a hard sheet with little ductility, it is annealed
either by batch annealing or continuous annealing. New casting technology is emerging
where thin sheet (under 1 mm) can be directly cast from the liquid through water-cooled,
rotating rolls that act as a mold as in continuous casting. This new process eliminates many
of the steps in conventional hot-rolled sheet processing. Plate steels are produced by hot
rolling a slab in a reversing roughing mill and a reversing ﬁnishing mill. Steel for railway
rails is hot rolled from a bloom in a blooming mill, a roughing mill, and one or more ﬁnishing
mills. Steel bars are produced from a heated billet that is hot rolled in a series of roughing
and ﬁnishing mills. Forged steels are produced from an ingot that is heated to forging tem-
perature and squeezed or hammered in a hydraulic press or drop forge. The processing
sequence in all these deformation processes can vary depending on the design, layout, and
age of the steel plant.
3 DEVELOPMENT OF STEEL PROPERTIES
In order to produce a steel product with the desired properties, basic metallurgical principles
are used to control three things:
6 Carbon and Alloy Steels
This means that the steel composition and processing route must be closely controlled in
order to produce the proper microstructure. The ﬁnal microstructure is of utmost importance
in determining the properties of the steel product. This section will explore how various
microstructures are developed and the unique characteristics of each microstructural com-
ponent in steel. The next section will discuss how alloy composition also plays a major role.
Iron–Carbon Equilibrium Diagram. Since most steels contain carbon, the basic principles
of microstructural development can be explained by the iron–carbon equilibrium diagram.
This diagram, shown in Fig. 1, is essentially a map of the phases that exist in iron at various
carbon contents and temperatures under equilibrium conditions. Iron is an interesting chem-
ical element in that it undergoes three phase changes when heated from room temperature
to liquid. For example, from room temperature to 912ЊC, pure iron exists as ferrite (also
called alpha iron), from 912 to 1394ЊC, it exists as austenite (gamma iron), from 1394 to
1538ЊC it exists as ferrite again (delta iron), and above 1538ЊC it is liquid. In other words,
upon heating, iron undergoes allotropic phase transformations from ferrite to austenite at
912ЊC, austenite to ferrite at 1394ЊC, and ferrite to liquid at 1538ЊC. Each transformation
undergoes a change in crystal structure or arrangement of the iron atoms in the crystal lattice.
It must be remembered that all chemical elements in their solid form have speciﬁc arrange-
ments of atoms that are essentially the basic building blocks in producing the element in the
form that we physically observe. These atomic arrangements form a latticework containing
billions of atoms all aligned in a systematic way. Some of these lattices have a cubic ar-
rangement, with an atom at each corner of the cube and another atom at the cube center.
This arrangement is called body-centered-cubic (bcc). Others have an atom at each corner
of the cube and atoms at the center of each face of the cube. This is called face-centered-
cubic (fcc). Other arrangements are hexagonal, some are tetragonal, etc. As an example, pure
iron as ferrite has a bcc arrangement. Austenite has a fcc arrangement. Upon heating, bcc
ferrite will transform to fcc austenite at 912ЊC. These arrangements or crystal structures
impart different properties to steel. For example, a bcc ferritic stainless steel will have prop-
erties much different from a fcc austenitic stainless steel, as described later in this chapter.
Since pure iron is very soft and of low strength, it is of little interest commercially.
Therefore, carbon and other alloying elements are added to enhance properties. Adding
carbon to pure iron has a profound effect on ferrite and austenite, discussed above. One way
to understand the effect of carbon is to examine the iron–carbon diagram (Fig. 1). This is a
binary (two-element) diagram of temperature and composition (carbon content) constructed
under near-equilibrium conditions. In this diagram, as carbon is added to iron, the ferrite
and austenite phase ﬁelds expand and contract depending upon the carbon level and tem-
perature. Also, there are ﬁelds consisting of two phases, e.g., ferrite plus austenite.
Since carbon has a small atomic diameter when compared with iron, it is called an
interstitial element because it can ﬁll the interstices between the iron atoms in the cubic
lattice. Nitrogen is another interstitial element. On the other hand, elements such as man-
ganese, silicon, nickel, chromium, and molybdenum have atomic diameters similar to iron
and are called substitutional alloying elements. These substitutional elements can thus replace
iron atoms at the cube corners, faces, or center positions. There are many binary phase
diagrams (Fe–Mn, Fe–Cr, Fe–Mo, etc.) and tertiary-phase diagrams (Fe–C–Mn, Fe–C–Cr,
etc.) showing the effect of interstitial and substitutional elements on the phase ﬁelds of ferrite
and austenite. These diagrams are found in the handbooks listed at the end of the chapter.
Being an interstitial or a substitutional element is important in the development of steel
properties. Interstitial elements such as carbon can move easily about the crystal lattice
whereas a substitutional element such as manganese is much more difﬁcult to move. The
movement of elements in a crystal lattice is called diffusion. Diffusion is a controlling factor
3 Development of Steel Properties 7
Figure 1 Iron–carbon binary-phase diagram. (Source: Steels: Heat Treatment and Processing Princi-
ples, ASM International, Materials Park, OH 44073-0002, 1990, p. 2.)
in the development of microstructure. Another factor is solubility, which is a measure of
how much of a particular element can be accommodated by the crystal lattice before it is
rejected. In metals when two or more elements are soluble in the crystal lattice, a solid
solution is created (somewhat analogous to a liquid solution of sugar in hot coffee). For
example, when added to iron, carbon has very limited solubility in ferrite but is about 100
times more soluble in austenite, as seen in the iron–carbon diagram in Fig. 2 (a limited
version of the diagram in Fig. 1). The maximum solubility of carbon in ferrite is about
3 Development of Steel Properties 9
0.022% C at 727ЊC while the maximum solubility of carbon in austenite is 100 times more,
2.11% C at 1148ЊC. At room temperature the solubility of carbon in iron is only about
0.005%. Any amount of carbon in excess of the solubility limit is rejected from solid solution
and is usually combined with iron to form an iron carbide compound called cementite. This
hard and brittle compound has the chemical formula Fe3C and a carbon content of 6.7%.
This is illustrated in the following two examples. The ﬁrst example is a microstructure of a
very low carbon steel (0.002% C), shown in Fig. 3a. The microstructure consists of only
ferrite grains (crystals) and grain boundaries. The second example is a microstructure of a
low-carbon steel containing 0.02% C, in Fig. 3b. In this microstructure, cementite can be
seen as particles at the ferrite grain boundaries. The excess carbon rejected from the solid
solution of ferrite formed this cementite. As the carbon content in steel is increased, another
form of cementite appears as a constituent called pearlite, which can be found in most carbon
steels. Examples of pearlite in low-carbon (0.08% C) and medium-carbon (0.20% C) steels
are seen in Figs. 4a and 4b. Pearlite has a lamellar (parallel-plate) microstructure, as shown
at higher magniﬁcation in Fig. 5, and consists of layers of ferrite and cementite. Thus, in
these examples, in increasing the carbon level from 0.002 to 0.02 to 0.08 to 0.20%, the
excess carbon is manifested as a carbide phase in two different forms, cementite particles
and cementite in pearlite. Both forms increase the hardness and strength of iron. However,
there is a trade-off; cementite also decreases ductility and toughness.
Pearlite forms on cooling austenite through a eutectoid reaction as seen below:
Austenite ↔ Fe C ϩ ferrite3
A eutectoid reaction occurs when a solid phase or constituent reacts to form two different
solid constituents on cooling (a eutectic reaction occurs when a liquid phase reacts to form
two solid phases). The eutectoid reaction is reversible on heating. In steel, the eutectoid
reaction (under equilibrium conditions) takes place at 727ЊC and can be seen on the iron–
carbon diagram (Fig. 1) as the ‘‘V’’ at the bottom left side of the diagram. A fully pearlitic
microstructure forms at 0.77% C at the eutectoid temperature of 727ЊC (the horizontal line
on the left side of the iron–carbon diagram). Steels with less than 0.77% C are called
hypoeutectoid steels and consist of mixtures of ferrite and pearlite with the amount of pearlite
increasing as the carbon content increases. The ferrite phase is called a proeutectoid phase
because it forms prior to the eutectoid transformation that occurs at 727ЊC. A typical example
of proeutectoid ferrite is shown in Fig. 6. In this photomicrograph, the ferrite (the white-
appearing constituent) formed on the prior austenite grain boundaries of hypoeutectoid steel
with 0.60% C. The remaining constituent (dark appearing) is pearlite. Steels between
0.77% C and about 2% C are called hypereutectoid steels and consist of pearlite with proeu-
tectoid cementite. Cementite forms a continuous carbide network at the boundaries of the
prior austenite grains. Because there is a carbide network, hypereutectoid steels are charac-
terized as steels with little or no ductility and very poor toughness. This means that in the
commercial world the vast majority of carbon steels are hypoeutectoid steels.
Thus, according to the iron–carbon diagram, steels that are processed under equilibrium
or near-equilibrium conditions can form (a) pure ferrite at very low carbon levels generally
under 0.005% C, (b) ferrite plus cementite particles at slightly higher carbon levels between
0.005% C and 0.022% C, (c) ferrite plus pearlite mixtures between 0.022% C and 0.77% C,
(d) 100% pearlite at 0.77% C, and (e) mixtures of pearlite plus cementite networks between
0.77% C and 2% C. The higher the percentage of cementite, the higher the hardness and
strength and lower the ductility and toughness of the steel.
Departure from Equilibrium (Real World). Industrial processes do not occur at equilibrium,
and only those processes that take place at extremely slow heating and cooling rates can be
considered near equilibrium, and these processes are quite rare. Therefore, under real con-
10 Carbon and Alloy Steels
Figure 3 (a) Photomicrograph of a very low carbon steel showing ferrite grains and (b) photo-
micrograph of a low-carbon steel showing ferrite grains with some cementite on the ferrite grain bound-
aries. (a) 500X and (b) 200X. Marshalls etch.
3 Development of Steel Properties 11
Figure 4 (a) Photomicrograph of an SAE/AISI 1008 steel showing ferrite grains and pearlite (dark)
and (b) photomicrograph of an SAE/AISI 1020 steel showing ferrite grains with an increased amount
of pearlite. (a) and (b) both 200X. 4% picral ϩ 2% nital etch.
12 Carbon and Alloy Steels
Figure 5 Scanning electron micrograph of pearlite showing the platelike morphology of the cementite.
5000X. 4% picral etch.
ditions, the iron–carbon diagram can only be used as a rough guideline since the equilibrium
transformation temperatures shift to lower temperatures on cooling and to higher tempera-
tures on heating. If steels are cooled at very fast rates, e.g., quenching in water, the iron–
carbon diagram can no longer be used since there is a major departure from equilibrium. In
fact, during the quenching of steel, new constituents form that are not associated with the
iron–carbon diagram. Therefore, at fast cooling rates the concept of time–temperature trans-
formation (TTT) diagrams must be considered. These diagrams are constructed under iso-
thermal (constant) temperature (called IT diagrams) or continuous-cooling conditions (called
CT diagrams). It is important to know how these diagrams are constructed so that we can
understand the development of nonequilibrium microstructures, which are so important in
carbon and alloy steels.
Isothermal Transformation Diagram. This diagram is formed by quenching very thin spec-
imens of steel in salt baths set at various temperatures. For example, thin specimens of
0.79% C steel can be quenched into seven different liquid salt baths set at 650, 600, 550,
500, 450, 400, and 200ЊC. The specimens are held for various times at each temperature
then pulled from the bath and quickly quenched in cold water. The result will be a diagram
called an isothermal transformation (IT) diagram, as shown in Fig. 7. The diagram is essen-
tially a map showing where various constituents form. For example, at 650ЊC, austenite (A)
begins to transform to pearlite if held in the bath for 10 s. The curve drawn through this
point is the pearlite transformation start temperature and is labeled beginning of transfor-
mation in Fig. 7. At about 100 s the pearlite transformation is ﬁnished. The second curve
represents the pearlite transformation ﬁnish temperature and is labeled the end of transfor-
3 Development of Steel Properties 13
Figure 6 Photomicrograph of a medium-carbon hypoeutectoid steel showing a pearlite matrix and
proeutectoid ferrite nucleating on the original (prior) austenite grain boundaries. 200X. 4% picral ϩ 2%
mation in Fig. 7. In this steel, pearlite forms at all temperatures along the start of the
transformation curve from 727ЊC (the equilibrium temperature of the iron–carbon diagram)
to 540ЊC, the ‘‘nose’’ of the curve. At the higher transformation temperatures, the pearlite
interlamellar spacing (the spacing between cementite plates) is very coarse and decreases in
spacing as the temperature is decreased, i.e., nose of the IT diagram is approached. This is
an important concept since a steel with a coarse pearlite interlamellar spacing is softer and
of lower strength than a steel with a ﬁne pearlite interlamellar spacing. Commercially, rail
steels are produced with a pearlitic microstructure, and it has been found that the ﬁner the
interlamellar spacing, the harder the rail and the better the wear resistance. This means that
rails will last longer in track if produced with the ﬁnest spacing allowable. Most rail pro-
ducers employ an accelerated cooling process called head hardening to obtain the necessary
conditions to achieve the ﬁnest pearlite spacing in the rail head (the point of wheel contact).
If the specimens are quenched to 450ЊC and held for various times, pearlite does not
form. In fact, pearlite does not isothermally transform at transformation temperatures (in this
case, salt pot temperatures) below the nose of the diagram in Fig. 7. The new constituent is
called bainite, which consists of ferrite laths with small cementite particles (also called
precipitates). An example of the microstructure of bainite is shown in Fig. 8. This form of
bainite is called upper bainite because it is formed in the upper portion below the nose of
the IT diagram (between about 540 and 400ЊC). Lower bainite, a ﬁner ferrite–carbide mi-
crostructure, forms at lower temperatures (between 400 and about 250ЊC). Bainite is an
important constituent in tough, high-strength, low-alloy steel.
If specimens are quenched into a salt bath at 200ЊC, a new constituent called martensite
will form. The start of the martensitic transformation is shown in Fig. 7 as Ms (at 220ЊC).
14 Carbon and Alloy Steels
Figure 7 Isothermal transformation diagram of SAE/AISI 1080 steel showing the beginning and end
of transformation curves with temperature and time. (Source: ASM Handbook, Vol. 1, Properties and
Selection: Irons, Steels, and High-Performance Alloys, ASM International, Materials Park, OH 44073-
0002, 1990, p. 128.)
Martensite is a form of ferrite that is supersaturated with carbon. In other words, because of
the very fast cooling rate, the carbon atoms do not have time to diffuse from their interstitial
positions in the bcc lattice to form cementite particles. An example of martensite is shown
in Fig. 9. Steel products produced with an as-quenched martensitic microstructure are very
hard and brittle, e.g., a razor blade. Most martensitic products are tempered by heating to
temperatures between about 350 and 650ЊC. The tempering process allows some of the
carbon to diffuse and form as a carbide phase from the supersaturated iron lattice. This
softens the steel and provides some ductility. The degree of softening is determined by the
tempering temperature and the time at the tempering temperature. The higher the temperature
and the longer the time, the softer the steel. Most steels with martensite are used in the
quenched and tempered condition.
Continuous-Cooling Transformation Diagram. The other more useful form of a time–
temperature transformation diagram is the continuous-cooling transformation (CT) diagram.
This differs from the IT diagram in that it is constructed by cooling small specimens at
various cooling rates and measuring the temperatures at which transformations start and ﬁnish
using a device called a dilatometer (a machine that measures dilation). Each phase transfor-
3 Development of Steel Properties 15
Figure 8 Photomicrograph of a low-alloy steel showing a bainitic microstructure. 500X. 4% picral ϩ
2% nital etch.
Figure 9 Photomicrograph of a low-alloy steel showing a martensitic microstructure. 1000X. 4%
picral ϩ HCl and 10% sodium metabisulfate etch.
16 Carbon and Alloy Steels
mation undergoes a distinct volume change (positive on cooling and negative on heating)
that can be measured by a sensitive length-measuring device in the dilatometer. A CT dia-
gram has similar features to the IT diagram shown in Fig. 7 but is produced by continuous
cooling rather than isothermal conditions. A continuous-cooling diagram is applicable for
most industrial processes and should be used in lieu of an IT diagram. A CT diagram can
also be constructed by quenching one end of a Jominy bar described below.
Hardenability Concept. In thick products, e.g., large-diameter bars, thick plates, and heavy
forgings, the through-thickness properties are achieved through hardenability. Hardenability
is the ability to induce depth of hardness in a steel product. The hardness level is obtained
by controlling the amount of martensite in the microstructure. To increase the depth of
hardness, certain alloying elements are added to the steel for increased hardenability. Ele-
ments, such as nickel, chromium, and molybdenum, shift the pearlite nose of the IT and CT
diagrams to the right (longer times). With the nose out of the way on cooling, martensite
can be formed over a wider range of cooling rates when compared with a steel without
There is a fairly simple test to measure the hardenability of steel called the Jominy test.
A 25.4-mm-diameter and 102-mm-long bar is austenitized to 845ЊC for 1 h and then water
quenched at one end of the bar. The quenching takes place in a specially designed ﬁxture
where the bar is suspended in the vertical position and water is directed against the machined
bottom end face of the bar. After quenching, parallel ﬂats 0.38 mm deep are machined on
opposite sides of the bar. Hardness is measured at 1.6-mm intervals from the1
quenched end. The hardness is plotted against depth from the quenched end to produce a
hardenability curve or band. A hardenability band for medium-carbon Society of Automotive
Engineers/American Iron and Steel Institute (SAE/AISI) 1045 steel is shown in Fig. 10a.
The two curves that form the band represent the maximum and minimum hardness values
from many Jominy tests. To illustrate the concept of hardenability, compare the hardenability
band for SAE/AISI 1045 steel to low-alloy SAE/AISI 4145 steel in Fig. 10b. These steels
are similar except that the low-alloy steel has chromium and molybdenum additions as shown
C Mn Si Cr Mo
0.42/0.51 0.50/1.00 0.15/0.35 — —
0.42/0.49 0.65/1.10 0.15/0.35 0.75/1.20 0.15/0.25
As can be seen from the hardenability bands, the higher manganese, chromium, and molyb-
denum additions in the SAE/AISI 4145 steel produced a much greater depth of hardness
than the plain-carbon steel. For example, a hardness of HRC 45 (Rockwell C scale) was
achieved at a depth of only 3–6.5 mm in the SAE/AISI 1045 steel compared with a hardness
of HRC 45 at a depth of 21–50 mm in the SAE/AISI 4145 steel. This low-alloy steel has
many times the depth of hardness or hardenability of the plain-carbon steel. This means that
a hardness of HRC 45 can be achieved in the center of a 100-mm-diameter bar of SAE/
AISI 4145 steel compared to a 10-mm-diameter bar of SAE/AISI 1045 steel (both water
quenched). The depth of hardness is produced by forming martensite near the quenched end
of the bar with mixtures of martensite and bainite further in from the end and eventually
bainite at the maximum depth of hardness. Hardenability is important since hardness is
roughly proportional to tensile strength. To convert hardness to an approximate tensile
strength, the conversion table in the American Society for Testing and Materials (ASTM)
E140 can be used. A portion of this table is
3 Development of Steel Properties 17
Figure 10 Hardenability curves for (a) SAE/AISI 1045 and (b) SAE/AISI 4145 showing depth of
hardness with distance from the quenched end of a Jominy bar (Source: ASM Handbook, Vol. 1, Prop-
erties and Selection: Irons, Steels, and High-Performance Alloys, ASM International, Materials Park,
OH 44073-0002, 1997, p. 487.)
C Scale Vickers
60 697 (654) —
55 595 560 2075
50 513 481 1760
45 446 421 1480
40 392 371 1250
35 345 327 1080
30 302 286 950
25 266 253 840
18 Carbon and Alloy Steels
Figure 10 (Continued)
This table also lists Vickers and Brinell hardness values, which are different types of hardness
tests. It can be seen that a hardness of HRC 45 converts to an approximate tensile strength
of 1480 MPa.
4 ROLE OF ALLOYING ELEMENTS IN STEEL
In the hardenability concept described in the previous section, alloying elements have a
profound effect on depth of hardness. Alloying elements also change the characteristics of
the iron–carbon diagram. For example, in the iron–carbon diagram (see Fig. 1) austenite
cannot exist below the eutectoid temperature of 727ЊC. However, there are steels where
austenite is the stable phase at room temperature, e.g., austenitic stainless steels and austenitic
manganese steels. This can only be achieved through alloying. There are, however, special
conditions where small amounts of austenite can be retained at room temperature during
rapid quenching of low-alloy steel. When this occurs, the austenite is too rich in alloying
elements to transform at room temperature and is thus retained as small regions in a mar-
tensitic microstructure. Because of this, it is called retained austenite. The retained austenite
can be transformed through tempering the steel.
4 Role of Alloying Elements in Steel 19
Figure 11 Iron–chromium equilibrium phase diagram. (Source: ASM Handbook, Vol. 20, Materials
Selection and Design, ASM International, Materials Park, OH 44073-0002, 1997, p. 365.)
In austenitic stainless steels, when nickel is added with chromium, the austenite phase
ﬁeld is expanded, allowing austenite to be stable at room temperature. The popular SAE/
AISI 304 austenitic stainless steel contains 18% Cr and 8% Ni. Austenitic manganese steel
(Hadﬁeld steel) contains 12% Mn with 1% C. The Mn and C allow austenite to be stable at
room temperature. Because of this ability, nickel and manganese are, therefore, called aus-
tenite stabilizers. Other elements are ferrite stabilizers, e.g., chromium, silicon, and molyb-
denum. A ferrite-stabilizing element expands the ferrite phase ﬁeld, and the austenite phase
ﬁeld is restricted within what is called a gamma loop (gamma, ␥, is the symbol for austenite).
A gamma loop can be seen in the iron–chromium equilibrium diagram in Fig. 11. The
gamma loop is shown at the left side of the diagram. According to this diagram, iron–
chromium alloys with 12.7% Cr or higher, the transformation from austenite (␥) to ferrite
(␣) does not occur and ferrite exists from room temperature to melting. Iron–chromium alloys
make up an important class of stainless steels called ferritic and martensitic stainless steels.
Each particular alloying element has an inﬂuence on the structure and properties of
steel. The following elements are important alloying elements in steel:
Carbon. Carbon is the most common alloying element in steel. It is inexpensive and has a
strong inﬂuence on hardness and strength. It is the basic and essential alloying element in
all plain-carbon, low-alloy, and tool steels. Carbon is an interstitial element that occupies
sites between the larger iron atoms in the bcc and fcc lattices. The inﬂuence of carbon on
the strength of iron can be seen in Fig. 12. Carbon can increase yield strength of pure iron
(0% C) with a strength of about 28–190 MPa. At 0.005% C, the maximum solubility of
carbon at room temperature the sevenfold increase in strength is due to interstitial solid
solution strengthening. Any excess carbon, above 0.005% C, will form an iron carbide com-
20 Carbon and Alloy Steels
Figure 12 Effect of carbon in solid solution on the yield strength of iron. (Source: ASM Handbook,
Vol. 20, Materials Selection and Design, ASM International, Materials Park, OH 44073-0002, 1997, p.
pound called cementite (Fe3C). Cementite can exist as a particle, as a component of lamellar
pearlite, or as a proeutectoid network on prior austenite grain boundaries in hypereutectoid
steel. Thus, carbon in the form of cementite has a further inﬂuence on the strength of steel,
as seen in Fig. 13. In this plot, the steels between 0.1% C and 0.8% C contain about 10–
100% pearlite. Yield strength peaks at about 425 MPa at 0.6% C whereas tensile strength
(ultimate strength) increases to 790 MPa at 0.8% C. These properties are for carbon steels
in the air-cooled condition. In a 0.8% C steel, a further increase in strength can be achieved
if faster cooling rates are used to produce a ﬁner pearlite interlamellar spacing. In a fully
pearlitic, head-hardened rail steel (accelerated cooled), the yield strength can increase to 860
MPa and tensile strength to 1070 MPa. Carbon also has a negative effect on properties, as
seen in Fig. 13. For example, the percent reduction in area (as well as total elongation not
shown) decreases with increasing carbon. The percent reduction in area is a measure of the
cross-sectional area change in a tensile specimen before and after fracture. Notch toughness
also decreases with carbon content, as seen in the decrease in upper shelf energy and the
increase in transition temperature. Shelf energy is the upper portion or upper shelf of a curve
of absorbed energy plotted from a Charpy test.
Manganese. Manganese is also an essential element in all carbon, low-alloy, and alloy steels.
Manganese has several roles as an alloying element. One role is to assure that all residual
sulfur is combined to form manganese sulﬁde (MnS). Manganese is generally added to steel
with a minimum manganese–sulfur ratio of 20Ϻ1. Without manganese the sulfur would com-
bine with iron and form iron sulﬁde (FeS), which is a brittle compound that lowers toughness
and ductility and causes a phenomenon called hot shortness. Hot shortness is a condition
where a compound (such as FeS) or insoluble element (such as copper) in steel has a low
melting point and thus forms an unacceptable cracklike surface condition during hot rolling.
Another role of manganese is in strengthening steel. Manganese is a substitutional element
and can replace iron atoms in the bcc or fcc lattice. Each 0.1% Mn added to iron will
increase the yield strength by about 3 MPa. Manganese also lowers the eutectoid transfor-
mation temperature and lowers the eutectoid carbon content. In large amounts (12% or
higher), manganese is an austenite stabilizer in alloy steels and forms a special class of steels
called austenitic manganese steels (also called Hadﬁeld manganese steels). These steels are
4 Role of Alloying Elements in Steel 21
Figure 13 Effect of carbon on the tensile and notched impact properties of ferrite–pearlite steels.
(Source: ASM Handbook, Vol. 20, Materials Selection and Design, ASM International, Materials Park,
OH 44073-0002, 1997, p. 367.)
used in applications requiring excellent wear resistance, e.g., in rock crushers and in railway
track connections where two rails meet or cross.
Silicon. Silicon is added to many carbon and low-alloy steels as a deoxidizer, i.e., it removes
dissolved oxygen from molten steel during the steel-reﬁning process. Oxygen is an undesir-
able element in steel because it forms oxide inclusions, which can degrade ductility, tough-
ness, and fatigue resistance. Silicon has a moderate effect on strengthening steel but is usually
not added for strengthening. Each 0.1% Si increases the yield strength of iron by about 8
MPa. It is a ferrite stabilizer and is found in some stainless steels. Silicon is also added to
steel for enhanced electrical properties, e.g., iron–silicon transformer steels at 3.25% Si.
These carbon-free steels have high magnetic permeability and low core loss.
Phosphorus. Phosphorus is considered a tramp or residual element in steel and is carefully
restricted to levels generally below 0.02%. However, like carbon, phosphorus is an interstitial
element that can substantially strengthen iron. For this reason, phosphorus is added to a
22 Carbon and Alloy Steels
special class of steels called rephosphorized steels for strength. Rephosphorized steels also
have enhanced machinability.
Sulfur. Sulfur is also considered a tramp element in steel and is usually restricted to below
about 0.02%. Although an element with a small atomic diameter, sulfur is not considered
an interstitial alloying element because it is insoluble in iron. However, as in the case of
phosphorus, sulfur is added to a special class of steels called resulfurized steels that have
improved machinability. These steels are called free-machining steels.
Copper. In most steels copper is considered a tramp (residual) element and is restricted to
levels below 0.04%. Copper, having a much lower melting point than iron, can create a
detrimental steel surface condition known as hot shortness. Although not generally added to
steel, there is a very special class of steels that contain high levels of copper to take advantage
of the precipitation of copper particles during aging (a tempering process). These copper
particles increase strength and hardness. Copper is also added to low-alloy steels for atmos-
pheric corrosion protection (these steels are called weathering steels). One problem with
copper in steel is that it cannot be oxidized and removed during steel reﬁning. Thus, over
time, the copper level of steel produced from steel scrap is slowly increasing.
Nickel. Nickel is an important element because of its positive effect on hardenability. Many
important low-alloy steels contain nickel for this reason. Nickel, being a substitutional ele-
ment in the iron lattice, has a small effect on increasing yield strength. Nickel, being an
austenite stabilizer, is also a vital element in austenitic stainless steels. Nickel is also im-
portant in steels for cryogenic applications and storage tanks for liqueﬁed hydrocarbon gases.
Nickel does not form a carbide and remains in solid solution.
Chromium. Like nickel, chromium has a positive effect on hardenability and is an important
alloying element in many low-alloy steels. For corrosion resistance, chromium is present in
all stainless steels as a solid solution element. In addition to hardenability and solid solution
effects, chromium forms several important chromium carbides that are necessary for wear
resistance in many tool steels and steels used for rolls in hot- and cold-rolling mills.
Molybdenum. Molybdenum is a potent hardenability element and is found in many low-
alloy steels. Molybdenum, like chromium, forms several types of carbides that are important
for wear-resistant applications, e.g., tool steels. Molybdenum is added to minimize temper
embrittlement in low-alloy steels. Temper embrittlement occurs when low-alloy steels are
tempered in the temperature range of 260–370ЊC. The embrittlement is caused by tramp
elements such as phosphorus that accumulate at the prior austenite grain boundaries and thus
weaken the boundaries. Adding molybdenum prevents the accumulation of these undesirable
elements at the boundaries. Molybdenum also enhances the creep strength of low-alloy steels
at elevated temperatures and is used in rotors and other parts of generators in electric power
plants. Creep is an undesirable process that allows steel to slowly elongate or creep under
load. Eventually the component will fail.
Vanadium. Although vanadium is a potent hardenability element, its most useful role is in
the formation of a vanadium nitride and vanadium carbide (it can also be in a combined
form of vanadium carbonitride). A very important role of vanadium is in microalloyed steels,
also called high-strength, low-alloy (HSLA) steels. These steels are strengthened by precip-
itation of vanadium nitrides and vanadium carbides (vanadium carbonitrides). The formation
of vanadium carbide is important for wear resistance. Vanadium carbide is much harder than
4 Role of Alloying Elements in Steel 23
iron carbide, chromium carbide, and molybdenum carbide. Vanadium is thus important in
high-speed tool steels, which are used as drill bits that retain their hardness as the tool heats
Tungsten. Tungsten is not an addition to low-alloy steels but is a vital alloying element in
high-speed tool steels where it forms hard tungsten carbide particles.
Aluminum. Aluminum is employed as a deoxidizer in steel and is generally used in con-
junction with silicon (also a deoxidizer). A deoxidizer removes undesirable oxygen from
molten steel. Once removed, the steel is called ‘‘killed.’’ Aluminum–silicon deoxidized
(killed) steels are known as ﬁne-grain steels. Another important role of aluminum is the
formation a aluminum nitride (AlN) precipitate. Many steels depend upon the formation of
AlN, especially steels used for sheet-forming applications requiring a high degree of form-
ability such as parts that require deep drawing. These steels are called drawing-quality
special-killed (DQSK) steels. The AlN precipitates help in the formation of an optimum
crystallographic texture (preferred orientation) in low-carbon sheet steels for these deep-
drawing applications. When aluminum combines with nitrogen to form AlN, the dissolved
interstitial nitrogen is lowered. Lower interstitial nitrogen (interstitial nitrogen is also called
free nitrogen) provides improved ductility. Aluminum can also substitute for silicon in elec-
trical steels for laminations in electric motors and transformer cores.
Titanium. Titanium is a strong deoxidizer but is usually not used solely for that purpose.
Titanium is important in microalloyed steels (HSLA steels) because of the formation of
titanium nitride (TiN) precipitates. Titanium nitrides pin grain boundary movement in aus-
tenite and thus provide grain reﬁnement. Another role of titanium is in steels containing
boron where a titanium addition extracts nitrogen from liquid steel so that boron, a strong
nitride former, remains in elemental form to enhance hardenability. Because of its afﬁnity
for both carbon and nitrogen, titanium is important in IF steels. Interstitial-free steels are an
important class of steels with exceptional formability. Titanium, being a strong carbide for-
mer, is used as a carbide stabilizer in austenitic stainless steels (AISI type 321), ferritic
stainless steels (AISI type 409, 439, and 444), and precipitation hardening stainless steels
(AISI type 600 and 635).
Niobium (Columbium). Niobium is also important in microalloyed (HSLA) steels for its
precipitation strengthening through the formation of niobium carbonitrides. Some microal-
loyed steels employ both vanadium and niobium. Because of its afﬁnity for both carbon and
nitrogen, niobium is an element found in some IF steels. Niobium is also added as a carbide
stabilizer (prevents carbides from dissolving and re-forming in undesirable locations) in some
austenitic stainless steels (AISI type 347, 348, and 384), ferritic stainless steels (AISI type
436 and 444), and precipitation hardening stainless steels (AISI type 630).
Tantalum. Because of its afﬁnity for carbon, tantalum, like niobium, is added as a carbide
stabilizer to some austenitic stainless steels (AISI type 347 and 348).
Boron. On a weight percent basis, boron is the most powerful hardenability element in steel.
A minute quantity of boron, e.g., 0.003%, is sufﬁcient to provide ample hardenability in a
low-alloy steel. However, boron is a strong nitride former and can only achieve its harden-
ability capability if in elemental form. Thus, boron must be protected from forming nitrides
by adding a sufﬁcient amount of titanium to ﬁrst combine with the nitrogen in the steel.
24 Carbon and Alloy Steels
Calcium. Calcium is a strong deoxidizer in steel but is not used for that purpose. In an
aluminum-deoxidized (killed) steel, calcium combines with sulfur to form calcium sulﬁde
particles. This form of sulﬁde remains as spherical particles as compared with manganese
sulﬁde, which is soft and elongates into stringers upon hot rolling. Thus, steels properly
treated with calcium do not have the characteristics associated with MnS stringers, i.e.,
property directionality or anisotropy.
Zirconium. Although expensive and rarely added to steel, zirconium acts like titanium in
forming zirconium nitride participates.
Nitrogen. Nitrogen is added to some steels, e.g., steels containing vanadium, to provide
sufﬁcient nitrogen for nitride formation. This is important in microalloyed steels containing
vanadium. Nitrogen, being an interstitial element like carbon, strengthens ferrite. A number
of austenitic stainless steels contain nitrogen for strengthening (AISI type 201, 202, 205,
304N, 304LN, 316N, and 316LN).
Lead. Lead is added to steel for enhanced machinability. Being insoluble in iron, lead par-
ticles are distributed through the steel and provide both lubrication and chip breaking ability
during machining. However, leaded steels are being discontinued around the world because
of the environmental health problems associated with lead.
Selenium. Selenium is added to some austenitic stainless steels (AISI type 303Se), ferritic
stainless steels (AISI type 430Se), and martensitic stainless steels (AISI type 416Se) for
improved machined surfaces.
Rare Earth Elements. The rare earth elements cerium and lanthanum are added to steel for
sulﬁde shape control, i.e., the sulﬁdes become rounded instead of stringers. It is usually
added in the form of mish metal (a metallic mixture of the rare earth elements).
Residual Elements. Tin, antimony, arsenic, and copper are considered residual elements in
steel. They are also called tramp elements. These elements are not intentionally added to
steel but remain in steel because they are difﬁcult to remove during steelmaking and reﬁning.
Steels made by electric furnace melting employing scrap as a raw material contain higher
levels of residual elements than steels made in an integrated steelmaking facility (blast
furnace–BOF route). Some electric furnace melting shops use direct-reduced iron pellets to
dilute the effect of these residuals.
Hydrogen. Hydrogen gas is also a residual element in steel and can be very deleterious.
Hydrogen is soluble in liquid steel and somewhat soluble in austenite. However, it is very
insoluble in ferrite and is rejected as atomic hydrogen (Hϩ
). If trapped inside the steel, usually
in products such as thick plate, heavy forgings, or railroad rail, hydrogen will accumulate
on the surfaces of manganese sulﬁde inclusions. When this accumulation takes place, mo-
lecular hydrogen (H2) can form and develop sufﬁcient pressure to create internal cracks. As
the cracks grow, they form what is termed hydrogen ﬂakes and the product must be scrapped.
However, if the product is slow cooled from the rolling temperature, the atomic hydrogen
has sufﬁcient time to diffuse from the product, thus avoiding hydrogen damage. Also, most
modern steelmakers use degassing to remove hydrogen from liquid steel.
5 Heat Treatment of Steel 25
5 HEAT TREATMENT OF STEEL
One of the very important characteristics of steel is the ability to alter the microstructure
through heat treatment. As seen in the previous sections, many different microstructural
constituents can be produced. Each constituent imparts a particular set of properties to the
ﬁnal product. For example, by quenching a steel in water, the steel becomes very hard but
brittle through the formation of martensite. By tempering the quenched steel, some ductility
can be restored with some sacriﬁce in hardness and strength. Also, superior wear properties
can be obtained in fully pearlitic microstructures, particularly if an accelerated cooling proc-
ess is employed to develop a ﬁne interlamellar spacing. Complex parts can be designed by
taking advantage of the formability and ductility of ferritic sheet steel through cold rolling
and annealing. The amount of pearlite in ferritic steel can be adjusted by carbon content and
cooling rate to produce a wide range of hardness and strength. In quenched and tempered
steels, a bainitic microstructure has a unique combination of high strength and toughness.
Thus steel, more than any other metallic material, can be manipulated through heat treatment
to provide a multiplicity of microstructures and ﬁnal properties. The common types of heat
treatment are listed below:
Annealing (Full Annealing). One of the most common heat treatments for steel is annealing.
It is used to soften steel and to improve ductility. In this process, the steel is heated into the
lower regions of the austenite phase ﬁeld and slow cooled to room temperature. The resulting
microstructure consists of coarse ferrite or coarse ferrite plus pearlite, depending upon carbon
and alloy content of the steel.
Normalizing. Steel is normalized by heating into the austenite phase ﬁeld at temperatures
somewhat higher than those used by annealing followed by air cooling. Many steels are
normalized to establish a uniform ferrite plus pearlite microstructure and a uniform grain
Spheroidizing. To produce a steel in its softest possible condition, it is usually spheroidized
by heating just above or just below the eutectoid temperature of 727ЊC and holding at that
temperature for an extended time. This process breaks down lamellar pearlite into small
spheroids of cementite in a continuous matrix of ferrite, as seen in Fig. 14. To obtain a very
uniform dispersion of cementite spheroids, the starting microstructure is usually martensite.
This is because carbon is more uniformly distributed in martensite than in lamellar pearlite.
The cementite lamella must ﬁrst dissolve and then redistribute the carbon as spheroids
whereas the cementite spheroids can form directly from martensite.
Process Annealing (Recrystallization Annealing). Process annealing takes place at temper-
atures just below the eutectoid temperature of 727ЊC. This treatment is applied to low-carbon,
cold-rolled sheet steels to restore ductility. In aluminum-killed steels, the recrystallized ferrite
will have an ideal crystallographic texture (preferred orientation) for deep drawing into com-
plex shapes such as oil ﬁlter cans and compressor housings. Crystallographic texture is
produced by developing a preferred orientation of the ferrite grains, i.e., the crystal axes of
the ferrite grains are oriented in a preferred rather than random orientation.
Stress Relieving. Steel products with residual stresses can be heated to temperatures ap-
proaching the eutectoid transformation temperature of 727ЊC to relieve the stress.
26 Carbon and Alloy Steels
Figure 14 Photomicrograph of a medium-carbon steel in the spheroidized condition. 500X. 4%
picral ϩ 2% nital etch.
Quenching. To produce the higher strength constituents of bainite and martensite, the steel
must be heated into the austenite phase ﬁeld and rapidly cooled by quenching in oil or water.
High-strength, low-alloy steels are produced by this process followed by tempering. It must
be noted that employing microalloying additions such as Nb, V, and Ti can also produce
HSLA steels. These microalloyed steels obtain their strength by thermomechanical treatment
rather than heat treatment.
Tempering. When quenched steels (martensitic steel) are tempered by heating to tempera-
tures approaching the eutectoid temperature of 727ЊC, the dissolved carbon in the martensite
forms cementite particles, and the steels become more ductile. Quenching and tempering are
used in a variety of steel products to obtain desired combinations of strength and toughness.
6 CLASSIFICATION AND SPECIFICATIONS OF STEELS
Since there are literally thousands of different steels, it is difﬁcult to classify them in a
simple straightforward manner. However, some guidelines can be used. For example, steels
are generally classiﬁed as carbon steel or alloy steel. A classiﬁcation system was developed
by the SAE as early as 1911 to describe these carbon and alloy steels. The AISI collaborated
with SAE to reﬁne the compositional ranges of the classiﬁcation that are used today. Re-
cently, a Uniﬁed Numbering System (UNS) was established that incorporates the SAE/AISI
Many steel products are purchased by speciﬁcations describing speciﬁc compositional,
dimensional, and property requirements. Speciﬁcation organizations such as ASTM have
6 Classiﬁcation and Speciﬁcations of Steels 27
developed numerous speciﬁcations for steel products and the testing of steel products. Some
speciﬁc product user groups in the United States have developed their own speciﬁcations,
e.g., the American Bureau of Ships (ABS) for ship plate and other marine products, Aero-
space Materials Speciﬁcations (AMS) for aerospace applications, the American Railway En-
gineering and Maintenance of Way Association (AREMA) for rail and rail products, the SAE
for automotive applications, and the American Society of Mechanical Engineers (ASME) for
steels produced to boiler code speciﬁcations. In Japan, there are standards developed by the
Japanese Industrial Standards (JIS) Committee of the Ministry of International Trade and
Industry. In the United Kingdom, there are the British Standards (BS) developed by the
British Standards Institute. In Europe, Germany has the Deutsches Institut fu¨r Normung
(DIN) standards, France the Association Francaise de Normalisation (AFNOR) standards,
and Italy the Ente Nazionale Italiano di Uniﬁcazione (UNI) standards.
Speciﬁcations can be as simple as a hardness requirement, i.e., ASTM A1 for rail steel
to elaborate compositional and property requirements as in ASTM A808, ‘‘High-strength
low-alloy carbon–manganese–niobium–vanadium steel of structural quality with improved
notch toughness.’’ Describing speciﬁc speciﬁcations is beyond the scope of this handbook,
but many of the key sources can be found in the Bibliography at the end of this chapter.
6.1 Carbon Steels
Carbon steels (also called plain-carbon steels) constitute a family of iron–carbon–manganese
alloys. In the SAE/AISI system, the carbon steels are classiﬁed as follows:
Nonresulfurized carbon steels 10xx series
Resulfurized steels 11xx series
Rephosphorized and resulfurized steels 12xx series
High-manganese carbon steels 15xx series
A four-digit SAE/AISI number is used to classify the carbon steels with the ﬁrst two digits
being the series code and the last two digits being the nominal carbon content in points of
carbon (1 point ϭ 0.01% C). For example, SAE/AISI 1020 steel is a carbon steel containing
0.20% C (actually 0.18–0.22% C). The chemical composition limits for the above SAE/
AISI 10xx series of carbon steels for semiﬁnished products, forgings, hot- and cold-ﬁnished
bars, wire, rods, and tubing are listed in SAE Materials Standards Manual (SAE HS-30,
1996). There are slight compositional variations for structural shapes, plates, strip, sheet, and
welded tubing (see SAE speciﬁcation J403). The SAE Manual gives the SAE/AISI number
along with the UNS number. The carbon level spans the range from under 0.06% C to
Because of the wide range in carbon content, the SAE/AISI 10xx carbon steels are the
most commonly used steels in today’s marketplace. All SAE/AISI 10xx series carbon steels
contain manganese at levels between 0.25 and 1.00%. For a century, manganese has been
an important alloying element in steel because it combines with the impurity sulfur to form
manganese sulﬁde (MnS). MnS is much less detrimental than iron sulﬁde (FeS), which would
form without manganese present. Manganese sulﬁdes are usually present in plain and low-
alloy steels as somewhat innocuous inclusions. The manganese that does not combine with
sulfur strengthens the steel. However, with the development of steelmaking practices to
produce very low sulfur steel, manganese is becoming less important in this role.
The SAE/AISI 11xx series of resulfurized steels contain between 0.08 and 0.33% sulfur.
Although in most steel, sulfur is considered an undesirable impurity and is restricted to less
28 Carbon and Alloy Steels
than 0.05%, in the SAE/AISI 11xx and 12xx series of steels, sulfur is added to form excess
manganese sulﬁde inclusions. These are the free-machining steels that have improved ma-
chinability over lower sulfur steels due to enhanced chip breaking and lubrication created
by the MnS inclusions.
The SAE/AISI 12xx series are also free-machining steels and contain both sulfur (0.16–
0.35%) and phosphorus (0.04–0.12%). The SAE/AISI 15xx series contain higher manganese
levels (up to 1.65%) than the SAE/AISI 10xx series of carbon steels.
Typical mechanical properties of selected SAE/AISI 10xx and 11xx series of carbon
steels are listed in the ﬁrst part of the table on pp. 20–23, Section 4, of the ASM Metals
Handbook, Desktop Edition, 1985, for four different processing conditions (as rolled, nor-
malized, annealed, and quenched and tempered). These properties are average properties
obtained from many sources, and thus this table should only be used as a guideline. The as-
rolled condition represents steel before any heat treatment was applied. Many applications
utilize steel in the as-rolled condition. As can be seen from the aforementioned ASM table,
yield and tensile strength is greater for steel in the normalized condition. This is because
normalizing develops a ﬁner ferrite grain size. Yield and tensile strength is lowest for steels
in the annealed condition. This is due to a coarser grain size developed by the slow cooling
rate from the annealing temperature. In general, as yield and tensile strength increase, the
percent elongation decreases. For example, in the ASM table, annealed SAE/AISI 1080 steel
has a tensile strength of 615 MPa and a total elongation of 24.7% compared with the same
steel in the normalized condition, with a tensile strength of 1010 MPa and a total elongation
of 10%. This relationship holds for most steel.
Special Low-Carbon Steels
These are the steels that are not classiﬁed in the aforementioned SAE table or listed in the
aforementioned ASM table. As mentioned earlier, carbon is not always beneﬁcial in steels.
These are special steels with carbon contents below the lower level of the SAE/AISI 10xx
steels. There are a number of steels that are produced with very low carbon levels (less than
0.002% C), and all the remaining free carbon in the steel is tied up as carbides. These steels
are known as IF steels, which means that the interstitial elements of carbon and nitrogen are
no longer present in elemental form in the iron lattice but are combined with elements such
as titanium or niobium as carbides and nitrides (carbonitrides). Interstitial-free steels are
required for exceptional formability, especially in applications requiring deep drawability.
Drawability is a property that allows the steel to be uniformly stretched (or drawn) in thick-
ness in a closed die without localized thinning and necking (cracking or breaking). An
example of a deep-drawn part would be a compressor housing for a refrigerator. With proper
heat treatment, IF steels develop a preferred crystallographic orientation that favors a high
plastic anisotropy ratio or r value. High r-value steels have excellent deep-drawing ability
and these steels can form difﬁcult parts. Another type of low-carbon steel is a special class
called DQSK steel. This type of aluminum-treated steel also has a preferred orientation and
high r value. The preferred orientation is produced by hot rolling the steel on a hot strip
mill followed by rapid cooling. The rapid cooling keeps the aluminum and interstitial ele-
ments from forming aluminum nitride particles (i.e., the Al and N atoms are in solid solution
in the iron lattice). After rolling, the steel is annealed to allow aluminum nitride to precipitate.
The aluminum nitride plays an important role in the development of the optimum crystal-
lographic texture. The DQSK steel is used in deep-drawing applications that are not as
demanding as those requiring IF steel.
A new family of steels called bake-hardening steels also have a low, but controlled
carbon content. These steels gain strength during the paint–bake cycle of automotive pro-
duction. Controlled amounts of both carbon and nitrogen combine with carbonitride-forming
elements such as titanium and niobium during the baking cycle (generally 175ЊC for 30
6 Classiﬁcation and Speciﬁcations of Steels 29
min). The precipitation of these carbonitrides during the paint–bake cycle strengthens the
steel by a process called aging.
Enameling steel is produced with as little carbon as possible because during the en-
ameling process, carbon in the form of carbides can react with the frit (the particles of
glasslike material that melts to produce the enamel coating) to cause defects in the coating.
Thus, steels to be used for enameling are generally decarburized in a special reducing at-
mosphere during batch annealing. In this process, the carbon dissipates from the steel. After
decarburization, the sheet steel is essentially pure iron. Enamel coatings are used for many
household appliances such as washers and dryers, stovetops, ovens, and refrigerators. Also,
steel tanks in most hot-water heaters have a glass (or enameled) inside coating.
Electrical steels and motor lamination steels are also produced with as low a carbon
content as possible. Dissolved carbon and carbides in these steels are avoided because the
magnetic properties are degraded. The carbides, if present in the steel, inhibit the movement
of the magnetic domains and lower the electrical efﬁciency. These steels are used in appli-
cations employing alternating current (AC) in transformers and electric motors. Most electric
motors for appliances and other applications have sheet steel stacked in layers (called lam-
inations) that are wound in copper wire. Electrical steels used for transformers contain sili-
con, which is added to enhance the development of a speciﬁc crystallographic orientation
that favors electrical efﬁciency.
6.2 Alloy Steels
Alloy steels are alloys of iron with the addition of one or more of the following elements;
carbon, manganese, silicon, nickel, chromium, molybdenum, and vanadium. The alloy steels
cover a wide range of steels, including low-alloy steels, stainless steels, heat-resistant steels,
and tool steels. Some alloy steels, such as austenitic stainless steels, do not contain intentional
additions of carbon. Silicon, when required, is added as a deoxidizer to the molten steel.
Nickel provides strength and assists in hardening the steel by quenching and tempering heat
treatment. This latter effect is called hardenability, which has been described earlier. Chro-
mium is found in stainless steels for corrosion resistance. Chromium and molybdenum also
assist in hardenability of the low-alloy steels. Vanadium strengthens the steel by forming
precipitates of vanadium carbonitride. Vanadium is also a potent hardenability element.
There is an SAE/AISI four-digit classiﬁcation system for the low-alloy steels. As in the
carbon steels, the ﬁrst two digits are for the alloy class and the last two (or three) digits are
for the carbon content. Because of the various combinations of elements, the system is more
extensive than that used for the carbon steels. The general SAE/AISI classiﬁcation system
for low-alloy steels is as follows:
Manganese steels 13xx series
Nickel steels 23xx, 25xx series
Nickel–chromium steels 31xx, 32xx, 33xx, and 34xx series
Molybdenum steels 40xx, 44xx series
Chromium–molybdenum steels 41xx series
Nickel–chromium–molybdenum steels 43xx and 47xx series
81xx, 86xx, 87xx, and 88xx series
93xx, 94xx, 97xx, and 98xx series
Nickel–molybdenum steels 46xx and 48xx series
30 Carbon and Alloy Steels
Chromium steels 50xx and 51xx series
50xxx, 51xxx, and 52xxx series
Chromium–vanadium steels 61xx series
Tungsten–chromium steels 71xxx, 72xx series
Silicon–manganese steels 92xx series
Boron steels xxBxx series
Leaded steels xxLxx series
The boron-containing steels are low-alloy steels with boron added in the amount of 0.0005–
0.003%. Boron is a strong hardenability element. The leaded steels contain 0.15–0.35% lead
for improved machinability (however, lead is no longer favored as an alloying addition
because of health concerns).
A table in the aforementioned SAE HS-30 lists the composition limits of most of the
families of the SAE/AISI low-alloy steels listed above. These steels are supplied in the form
of bar, plate, and forged products and are usually heat treated to obtain speciﬁc mechanical
properties, especially high strength and toughness. Mechanical properties of selected SAE/
AISI low-alloy steels in the as-rolled, annealed, normalized and quenched and tempered
conditions are listed in the aforementioned ASM table. These properties are average prop-
erties and should only be used as a guideline. For example, SAE/AISI 4340 steel is usually
heat treated by heating the component to 950–1000ЊC followed by quenching in oil. The
component is then tempered at a temperature between 205 and 650ЊC. According to the
aforementioned ASM table, this nickel–chromium–molybdenum steel in the quenched and
tempered condition (tempered at 205ЊC) can achieve a yield strength of 1675 MPa and a
tensile strength of 1875 MPa. Quenched and tempered low-alloy steels are used in a large
number of applications requiring high strength and good toughness. Note that in the annealed
condition, SAE/AISI 4340 steel has a yield strength of only 745 MPa.
Other Low-Alloy Steels
There are a number of important steels that do not ﬁt into the SAE/AISI classiﬁcation system
described above. Such classes are the microalloyed steels also called HSLA steels, dual-
phase steels, trip steels, and high-performance steels.
Microalloyed (High-Strength, Low-Alloy) Steels. Microalloying is a term applied to steels
that contain small additions of alloying elements that retard austenite recrystallization and
pin austenite grain boundary movement by the formation of small carbide and/or nitride
precipitates. These elements include vanadium, niobium, and titanium. These HSLA steels
are produced for a variety of plates, structural shapes, bars, and sheet applications with yield
strength varying from 290 to 690 MPa. These steels are covered under numerous SAE and
ASTM speciﬁcations. The SAE high-strength, low-alloy steels are covered under speciﬁca-
tions J410, J1392, and J1442 and the ASTM high-strength, low-alloy steels are covered
under various speciﬁcations, including A242, A440, A441, A572, A588, A606, A607, A618,
A633, A656, A690, A709, A714, A715, A808, A812, A841, A860, and A871. These HSLA
steels have found wide application in areas such as bridge construction (structural beams),
off-shore oil and natural gas platforms, ship hull and deck plate, and electrical transmission
towers and poles. In the automobile, HSLA steels are used for safety (ultrahigh-strength
impact door beams and energy-absorbing bumper assemblies) and for increasing fuel econ-
omy through thinner (lighter weight) chassis structural sections. Microalloyed HSLA steels
are also employed in large-diameter gas transmission pipelines.
6 Classiﬁcation and Speciﬁcations of Steels 31
Dual-Phase Steels. A relatively recent development, dual-phase steels are produced by rap-
idly cooling a medium-carbon steel, containing vanadium or molybdenum, from the two-
phase ferrite plus austenite region. The austenite transforms into islands of martensite
(stabilized at room temperature by the V and Mo additions) in a ferrite matrix. Depending
upon the alloy content, the martensite islands can also contain austenite that is retained below
the transformation temperature (called retained austenite). Thus, dual-phase steel may contain
both martensite and austenite as a second phase (called MA constituent). The unique char-
acteristic of dual-phase steels is the continuous yielding behavior during deformation; i.e.,
there is a lack of a yield point during deformation. This provides increased uniform elon-
gation and work hardening so that those components or parts produced from dual-phase steel
actually gain strength during the forming operation. Dual-phase steels are being applied in
applications such as automobile wheel rims and wheel disks. Because of their energy-
absorbing characteristics, dual-phase steels are being used in critical locations of the auto-
mobile for safety to protect the occupants in the event of a crash.
Trip Steels. Similar to dual-phase steels, trip steels have emerged as an energy-absorbing
high-strength steel for the automobile. The term ‘‘trip’’ is derived from the mechanism of
transformation induced plasticity. These steels contain a high percentage of retained austenite
(10–15%). The austenite transforms to martensite during the forming of the part, thus pro-
viding enhanced formability or transforms upon impact in a crash.
High-Performance Steels. There are a number of high-performance steels that are used in
critical applications. These low-alloy steels, such as HY80 and HY100, are used in appli-
cations requiring high strength and excellent toughness. The ‘‘80’’ and ‘‘100’’ in the codes
represent the minimum yield strength in ksi units. Another family of low-alloy steels is used
in heat exchangers, high-temperature piping, and boiler applications. These steels, like
2 Cr–1% Mo, ﬁnd wide use in these applications. Other high-performance steels are the1
Ni–Cr–Mo steels used as rotors for large steam generators and motors in electric power
plants. These steels must withstand temperatures of superheated steam and must maintain
high strength, superior toughness, as well as high fatigue strength and creep resistance. The
Ni–Cr–Mo–V steels are also used in pressure vessels in nuclear reactors.
Higher Alloy Steels
There is a distinction between the low-alloy steels described above and the higher alloy
steels (usually containing over 8% alloying elements). The higher alloy steels include stain-
less steels, tool steels, heat-resistant steels, wear-resistant steels, and ultrahigh-strength steels.
Stainless Steels. Stainless steels are corrosion-resistant steels that contain at least 10.5%
chromium. Chromium is unique in that it forms a passive layer on the steel surface that
provides protection from corrosion. There are basically ﬁve types of stainless steels: austen-
itic, ferritic, duplex, martensitic, and precipitation hardening steels. These ﬁve types of stain-
less steel have a somewhat simpliﬁed classiﬁcation system as follows:
Austenitic stainless steels with low nickel 2xx series
Austenitic stainless steels 3xx series
Ferritic stainless steels 4xx series
Duplex stainless steel 329
Martensitic stainless steels 4xx series
Precipitation strengthening stainless steels 6xx (xx-x PH)
32 Carbon and Alloy Steels
The classiﬁcation system is different for the stainless steels than the system for SAE/AISI
low-alloy steels in that the last two digits (xx) do not represent the carbon content and have
no particular compositional meaning. Unfortunately, the classiﬁcation system has some con-
fusion with the ferritic and martensitic stainless steels both of the 4xx series. The 2xx series
of austenitic stainless steels were developed during the 1950s when nickel became scarce.
In these steels, manganese and nitrogen were substituted for the lower nickel level in order
to maintain strength. Each type of stainless steel is expanded upon below:
AUSTENITIC STAINLESS STEELS. Austenitic stainless steels have sufﬁcient alloying to stabi-
lize austenite at room temperature. These steels being austenitic are nonmagnetic. Austenitic
stainless steels have excellent low-temperature toughness, weldability, and corrosion resis-
tance. On the other hand, they have relatively low yield strength and can only be strengthened
by cold working the steel, by precipitation hardening, or by interstitial or substitutional solid
The table on pp. 15.1–15.4 of the ASM Metals Handbook, Desktop Edition, 1985, lists
the composition limits of the austenitic stainless steels. In general, the 3xx series are iron–
chromium–nickel alloys that contain 16–26% chromium and 6–22% nickel. The popular
type 304 austenitic stainless steel contains 18–20% Cr and 8–12% Ni and is often referred
to as ‘‘18-8’’ stainless steel for the chromium and nickel content. There are many compo-
sitional variations of austenitic stainless steels. The following list summarizes these varia-
201 Low nickel replaced with manganese and nitrogen
202 Higher Mn than 201
205 Higher Mn and N than 202
301 Lower Ni and Cr to increase work-hardening ability
302 General-purpose 18–8 stainless steel
302B Scaling resistance improved with Si
303 Enhanced machinability with a S addition
303Se Improved machined surfaces with a selenium addition
304 Popular 18–8 stainless steel, lower C than 302
304L Low-carbon 304 for improved corrosion resistance
304LN Low-carbon 304 with nitrogen added for strength
304H Higher carbon 304
304Cu Copper added for improved cold working
304N Nitrogen added for strength
305 Higher Ni for reduced work hardening
308 Higher Cr and Ni for weldability
309 High Cr and Ni for heat resistance
309S Lower carbon 309
309Cb Niobium (columbium) added
310 Higher Cr and Ni than 309 for improved heat resistance
310S Lower carbon 310
310Cb Niobium (columbium) added
314 Higher Si for improved heat resistance
6 Classiﬁcation and Speciﬁcations of Steels 33
316 Mo added for improved corrosion resistance
316F Higher S and P for machinability
316L Lower C for improved corrosion resistance and weldability
316LN Lower C and higher nitrogen (for strength)
316H Higher carbon 316
316N Nitrogen added for strength
316Ti Titanium added
316Cb Niobium (columbium) added
317 Higher Cr and Mo for improved corrosion resistance
317L Low-carbon 317 for improved weldability
321 Titanium added to minimize Cr carbide precipitation
330 High Ni to minimize carburization and improve thermal shock
347 Nb and Ta added to minimize Cr carbide precipitation
347H Higher carbon 347
348 Ta and Co added for restricted nuclear applications
348H Higher carbon 348
384 Higher Ni for decreased work hardening
The limiting of carbon is important in austenitic stainless steels. When heated, carbon forms
chromium carbide that precipitates on the austenite grain boundaries and produces a con-
dition known as sensitization. Because the chromium is tied up as carbide, the chromium
adjacent to the boundaries will be depleted in chromium and corrosion can take place.
Sensitization is reversible by heating the steel to temperatures between 1040 and 1150ЊC
followed by rapid cooling to room temperature. The high temperature dissolves the carbides
and the rapid cooling prevents reprecipitation of the carbides. More on austenitic stainless
steel can be found in Chapter 2.
FERRITIC STAINLESS STEELS. The ferritic stainless steels are basically iron–chromium alloys
with chromium ranging from 10.5 to 27%. The compositional limits for the ferritic stainless
steels are listed in the aforementioned ASM table. Nickel is absent in ferritic stainless steels
except for minor amounts, i.e., less than 1%, in some alloys. These steels have a micros-
tructure of ferrite at room temperature and are magnetic. Type 409 stainless steel with the
lowest chromium level (10.5–11.75%) is the least expensive of the ferritic stainless steel
series and is used for automotive exhaust systems because it far outlasts carbon steel in that
application. There are fewer variations of ferritic stainless steels than austenitic stainless
steels. The ferritic stainless steels are listed below:
405 Low Cr with Al added
409 Low Cr, for automotive exhaust applications
429 Slightly less Cr, better weldability
430 General-purpose ferritic stainless steel
430F Free machining with higher S and P
430Se Selenium added for improved machined surfaces
434 Mo added for improved corrosion resistance
34 Carbon and Alloy Steels
436 Mo, Nb, and Ta added for corrosion and heat resistance
439 Low C, Ti added to minimize sensitization
442 Higher Cr for improved oxide scaling resistance
444 Low C, Mo for corrosion resistance, Ti and Nb for sensitization
446 Highest Cr for improved scaling resistance
Ferritic stainless steels are described in more detail in Chapter 2.
DUPLEX STAINLESS STEELS. Type 329 is an iron–chromium alloy with 2.5–5% nickel and
1–2% molybdenum that has a mixed (duplex) microstructure of approximately equal per-
centages of ferrite and austenite. There are many more duplex stainless steels that have
priority compositions and trade names (see Bibliography at the end of chapter). The corrosion
characteristics of these duplex stainless steels are similar to austenitic stainless steels. How-
ever, they have higher strength and better resistance to stress–corrosion cracking than aus-
tenitic stainless steels. Duplex stainless steels are discussed in Chapter 2.
MARTENSITIC STAINLESS STEELS. To produce martensite in a stainless steel, the alloy must
be transformed from the austenite phase ﬁeld. According to the equilibrium phase diagram,
this means that they have restricted chromium levels within the range required to form the
gamma loop where austenite exists (see Fig. 11). The gamma loop is the region between
800 and 1400ЊC and 0 and 12.7% Cr in Fig. 11. Since austenite only exists in this restricted
region, the steel must be heated within this temperature range and quenched to room tem-
perature to form martensite. Martensitic stainless steels contain added carbon, which expands
the gamma loop to allow higher chromium contents to be used. Because they can be heat
treated, the martensitic stainless steels generally have higher strength than the austenitic and
ferritic stainless steels. The martensitic stainless steels are listed below:
403 Select quality for highly stressed parts
410 General-purpose martensitic stainless steel
414 Ni added for improved corrosion
416 Higher P and S for improved machinability
416Se Se added for improved machined surfaces
420 Higher C for increased strength
420F Free machining with higher P and S
422 Mo, V, and W added for increased strength and toughness
431 Higher Cr, Ni added for improved corrosion resistance
440A Highest Cr, C added for increased hardness
440B Highest Cr, more C added for increased hardness/toughness
440C Highest Cr, highest C for increased hardness/toughness
501 Low Cr, Mo added
502 Low C, Mo added
The compositional ranges for the martensitic stainless steels are shown in the aforementioned
ASM table. Martensitic stainless steels are discussed in the next chapter.
6 Classiﬁcation and Speciﬁcations of Steels 35
PRECIPITATION HARDENING STAINLESS STEELS. The precipitation hardening stainless steels
are iron–chromium–nickel alloys that develop high strength and toughness through additions
of Al, Ti, Nb, V, and/or N, which form precipitates during an aging heat treatment. The
base microstructures of precipitation hardening stainless steels can be either martensitic
or austenitic depending upon composition and processing. Some selected grades are listed
600 Austenitic grade with Mo, Al, Ti, V, and B added
630 Martensitic grade with Cu and Nb added
631 Austenitic grade with Al added
633 Austenitic grade with Mo and N added
635 Martensitic grade with Al and Ti added
The compositional ranges of the precipitation hardening stainless steels are listed in the
aforementioned ASM table.
OTHER STAINLESS STEELS. There are many stainless steels that do not fall within the AISI
classiﬁcation system. These steels have proprietary compositions and trade names. Details
of many of these steels can be found in Chapter 2 and in the Bibliography at the end of this
Tool Steels. Tool steels are alloy steels that are used to cut or machine other materials. Tool
steels contain various levels of Cr, Ni, Mo, W, V, and Co. The categories of tool steels are:
M series Molybdenum high-speed steels
T series Tungsten high-speed steels
Cr series Chromium hot-work steels
H series Molybdenum hot-work steels
A series Air-hardening medium-alloy cold-work steels
D series High-carbon high-chromium cold-work steels
O series Oil-hardening cold-work steels
S series Shock-resistant steels
L series Low-alloy special-purpose tool steels
P series Low-carbon mold steels
W series Water-hardening tool steels
The compositional ranges of the various tool steels are listed in the table on pp. 758–759
of the ASM Metals Handbook, Vol. 20, 10th Edition, 1997. The high-speed steels are used
in high-speed cutting tools such as drill bits. The hot-work tool steels are used in operations
that utilize dies for punching, shearing, and forming materials at elevated temperatures, and
the cold-work steels are used in similar operations at room temperature.
Heat-Resistant Steels. The upper temperature limit for use of carbon steels is about 370ЊC
because of excessive oxidation and loss of strength. However, there are a number of alloy
steels, called heat-resistant steels, that can be used at temperatures of 540–650ЊC. These
steels include some of the ferritic stainless steels (405, 406, 409, 430, 434, and 439),
36 Carbon and Alloy Steels
quenched and tempered martensitic stainless steels (403, 410, 416, 422, and 431), precipi-
tation hardening martensitic stainless steels (15-5 PH, 17-4 PH, and PH 13-8 Mo), precipi-
tation hardening semiaustenitic stainless steels (AM-350, AM-355, 17-7 PH, and PH 15-7
Mo), and austenitic stainless steels (404, 309, 310, 316, 317, 321, 347, 202, and 216). In
addition to the stainless steels, there are a number of proprietary alloys containing various
levels of Cr, Ni, Mo, Nb, Ti, Cu, Al, Mn, V, N, or Si. The properties that are important to
heat-resistant steels are creep and stress rupture. Creep is time-dependent strain occurring
under stress. In more common terms creep is elongation or sagging of a part over time at
elevated temperature. Stress rupture is a measure of the elevated temperature durability of
material. These steels are generally speciﬁed under the ASME Boiler and Pressure Vessel
Wear-Resistant Steels (Austenitic Manganese Steels). An important series of alloy steels are
the austenitic manganese steels that contain 1.2% carbon and a minimum of 11% manganese.
These steels, invented by Sir Robert Hadﬁeld in 1882, are wear resistant and tough. Because
they are difﬁcult to hot work, these steels are usually cast into the ﬁnal product form. The
chemical compositional ranges for some selected austenitic manganese steels (ASTM A128)
are listed below:
Grade C Mn Cr Mo Ni Si
A 1.55–1.35 11 (min) — — — 1 (max)
B1 0.9–1.05 11.5–14 — — — 1 (max)
C 1.05–1.35 11.5–14 1.5–2.5 — — 1 (max)
D 0.7–1.3 11.5–14 — — 3–4 1 (max)
E1 0.7–1.3 11.5–14 — 0.9–1.2 — 1 (max)
The carbon addition is necessary to maintain an austenitic microstructure at room tempera-
ture. All grades must be heat treated by solution annealing at 1010–1090ЊC for 1–2 h per
25 mm of thickness followed by rapid water quenching. Because these alloys work harden
during use, they are used in applications involving earthmoving (bucket blades), mining and
quarrying (rock crushers), and railway trackwork (frogs, switches, and crossings).
MARAGING STEEL. Another important series of alloy steels are the maraging steels. They
are considered ultrahigh-strength steels because they can be heat treated to yield strength
levels as high as 2.5 GPa. They also have excellent ductility and toughness. There are
basically four grades that are produced to strength levels between 1.4 and 2.5 GPa.
Grade Ni Co Mo Ti Al
18Ni (200) 18 8.5 3.3 0.2 0.1
18Ni (250) 18 8.5 5.0 0.4 0.1
18Ni (300) 18 9.0 5.0 0.7 0.1
18Ni (350) 18 12.5 4.2 1.6 0.1
The numbers in parentheses represent the nominal yield strength level in ksi. All maraging
steels must be heat treated to achieve the desired properties. The heat treatment cycle for
the 18Ni (200), 18Ni (250), and 18Ni (300) grades requires a solution treatment at 820ЊC
for 1 h per 25 mm of thickness, cooling to room temperature, and an aging treatment at
480ЊC for 4 h. The 18Ni (350) grade has an extended aging time of 12 h. The heat treatment
develops a martensitic microstructure on cooling from austenite at 820ЊC. The aging step
precipitates intermetallic compounds, e.g., Ni3Mo, that strengthen the martensitic matrix.
Maraging steels can be machined before the aging treatment and have good weldability and
excellent fracture toughness. They have found applications in missile and aircraft parts that
require exceptional performance.
MUSIC WIRE. One of the strongest steel products commercially available is music wire.
These wires can achieve levels of tensile strength approaching 5 GPa. The steel is basically
SAE/AISI 1080. To obtain the ultrahigh-strength levels, rods of SAE/AISI 1080 are iso-
thermally transformed to ﬁne pearlite in a process known as patenting. The rods are then
cold drawn to wire using large reductions in wire diameter through each die. The cold
reduction forces the ferrite and cementite in the microstructure to align in a preferred ori-
entation or ﬁber texture. The wires are used in musical instruments where they can be
stretched under high tension to achieve certain musical notes. Ultrahigh-strength wires are
also used to strengthen the rubber in automobile tires.
Steel is one of the most versatile materials in today’s society. It can be produced with a
wide range of properties and is used in millions of applications. For example, stainless steels
are used for their corrosion resistance, interstitial-free steels are used for their excellent
formability characteristics, iron–silicon alloys are used for their electrical properties, austen-
itic manganese steels are used for their wear and abrasion resistance, microalloyed steels are
used for their high strength, patented and cold-drawn eutectoid steel wires are used for their
ultrahigh strength, dual-phase and trip steels are used for their energy absorption capability
in a vehicle collision, and tool steels are used for their outstanding ability to cut and machine
other materials. No other material can span such a range of properties and characteristics.
ASM Metals Handbook, Properties and Selection: Irons, Steels and High Performance Alloys, Vol. 1,
10th ed., ASM International, Materials Park, OH, 1990.
ASM Metals Handbook, Materials Selection and Design, Vol. 20, 10th ed., ASM International, Materials
Park, OH, 1997.
ASM Metals Handbook, Desk Edition, 2nd ed., ASM International, Materials Park, OH, 1998.
ASM Specialty Handbook—Stainless Steels, ASM International, Materials Park, OH, 1994.
ASM Specialty Handbook—Carbon and Alloy Steels, ASM International, Materials Park, OH, 1996.
Engineering Properties of Steel, ASM International, Materials Park, OH, 1982.
Stahlschlu¨ssel (Key to Steel), 18th ed., Verlag Stahlschlu¨ssel Wegst GMBH, Marburg, 1998.
Worldwide Guide to Equivalent Irons and Steels, 4th ed., ASM International, Materials Park, OH, 2000.
Beddoes, J., and J. G. Parr, Introduction to Stainless Steels, 3rd ed., ASM International, Materials Park,
38 Carbon and Alloy Steels
Brooks, C. R., Principles of the Heat Treatment of Plain Carbon and Low Alloy Steels, ASM Interna-
tional, Materials Park, OH, 1996.
Krauss, G., Steels—Heat Treatment and Processing Principles, ASM International, Materials Park, OH,
Honeycombe, R., and H. K. D. H. Bhadeshia, Steels: Microstructures and Properties, 2nd ed., Wiley,
New York, 1996.
Roberts, G., G. Krauss, and R. Kennedy, Tool Steels, 10th ed., ASM International, Materials Park, OH,
Speciﬁcations on Steel Products
Annual Book of ASTM Standards, Vol. 01.01, Steel—Piping, Tubing, Fittings, ASTM, West Consho-
hocken, PA, 2001.
Annual Book of ASTM Standards, Vol. 01.02, Ferrous Castings, Ferroalloys, Shipbuilding, ASTM, West
Conshohocken, PA, 2001.
Annual Book of ASTM Standards, Vol. 01.03, Steel—Plate, Sheet, Strip, Wire, ASTM, West Consho-
hocken, PA, 2001.
Annual Book of ASTM Standards, Vol. 01.04, Steel—Structural, Reinforcing, Pressure Vessel, Railway,
ASTM, West Conshohocken, PA, 2001.
Annual Book of ASTM Standards, Vol. 01.05, Steel—Bars, Forgings, Bearing, Chain, Springs, ASTM,
West Conshohocken, PA, 2001.
Annual Book of ASTM Standards, Vol. 01.06, Coated Steel Products, ASTM, West Conshohocken, PA,
SAE Materials Standards Manual, SAE HS-30, Society of Automotive Engineers, Warrendale, PA, 2000.
1 EFFECT OF ALLOYING 39
2 SOME FORMS OF CORROSION 43
2.1 General Corrosion 43
2.2 Stress–Corrosion Cracking 44
2.3 Pitting Corrosion 45
2.4 Crevice Corrosion 45
2.5 Intergranular Corrosion 46
2.6 Galvanic Corrosion 47
3 AOD, DUAL CERTIFICATION,
AND CHEMISTRY CONTROL 47
4 AVAILABILITY 49
5 FERRITIC STAINLESS STEEL 49
6 MARTENSITIC STAINLESS
8 DUPLEX STAINLESS STEELS 51
9 AUSTENITIC STAINLESS AND
NICKEL ALLOYS 51
10 WELDING 53
10.1 Carbon versus Stainless Steel 53
10.2 Austenitic Alloys 55
10.3 Duplex Stainless Steels 57
10.4 High-Molybdenum Alloys 57
WEB SITES 58
Stainless steels are those alloys of iron and chromium, with or without other elements,
containing at least 11% chromium. This is the minimum amount of chromium necessary to
form a stable, passive chromium oxide ﬁlm. It is this ﬁlm that is the basis for the corrosion
resistance of all stainless, and most nickel-base, corrosion-resistant alloys.
There are six basic classiﬁcations of stainless steels: ferritic, martensitic, martensitic age
hardening, duplex austenitic–ferritic, and austenitic. The most commonly produced of these
are the ferritics 409 for automotive applications and 430 for corrosion-resistant/decora-
tive uses, the martensitic grade 410, and the age-hardening martensitic 17-4PH᭨
. Of the
austenitic–ferritic duplex grades, alloy 2205 is the most broadly available. The two most
used austenitic stainless grades are 304L and 316L. A number of ‘‘superaustenitics’’ use
nitrogen to maintain an austenitic structure with relatively high molybdenum, some 6%, and
moderate nickel, 18–25%. Of the higher nickel grades alloys 825 and 20 are used for sulfuric
acid and general chemical processing. The most commonly used of the very high nickel
alloys is C-276. The austenitic stainless steels form a continuum with the nickel-base heat-
and corrosion-resistant alloys. They are distinguished on the basis of nickel content by ar-
bitrary or commercial deﬁnitions. There is no recognized metallurgical deﬁnition of where
stainless ends and nickel base begins.
1 EFFECT OF ALLOYING ELEMENTS
The corrosion behavior of the alloying elements in pure form inﬂuences the corrosion prop-
erties of the alloys made from them.
Mechanical Engineers’ Handbook: Materials and Mechanical Design, Volume 1, Third Edition.
Edited by Myer Kutz
Copyright 2006 by John Wiley & Sons, Inc.
40 Stainless Steels
Chromium is the ﬁrst example, with outstanding corrosion resistance in the passive state.
In solutions of neutral pH, dissolved oxygen from the air is sufﬁcient to maintain passivity.
But in low-pH solutions, stronger oxidizing agents must be present and halogen or sulfuric
acids absent in order to stabilize the passive condition. Chromium metal is not resistant to
corrosion by reducing acids.1
Some examples, from Uhlig,1
of corrosion resistance of electrodeposited chromium are
Temperature Corrosion Rate
Acid or Salt (%) ЊC ЊF mm/yr mils/yr
Acetic 10 58 136 0.39 15
Ferric chloride 10 58 136 0.41a
Fomic 10 58 136 30 1,200
Hydrobromic 10 58 136 4.7 186
Hydroﬂuoric 10 12 54 25 1,000
Perchloric 10 58 136 0.86 42
Phosphoric 10 58 136 0.28 34
Sulfuric 10 12 54 0.86 11
Sulfuric 10 58 136 250 10,000
Sulfuric 100 12 34 0.76 30
Sulfuric 100 58 136 1.8 69
Pitting occurred; this number does not reﬂect uniform corrosion.
Three points can be made from these data. First, chromium as an alloying element is
not particularly effective in promoting resistance to reducing or halogen acids. Second, in
solutions of some halogen salts the passive layer was maintained by oxygen dissolved in the
solution. Third, sulfuric acid behaves as a reducing acid in lower concentrations but as an
oxidizing acid in concentrated form. When selecting alloys to resist sulfuric acid, one must
bear this in mind.
Stainless steels containing only chromium and iron, speciﬁcally the ferritic and marten-
sitic stainless steels, likewise have poor resistance to sulfuric acid solutions but may resist
nitric acid. These chromium–iron alloys are not resistant to corrosion by halogen acids or
chloride salts. Those ferritic alloys that do have good to excellent chloride pitting resistance,
such as E-Brite᭨
, gain that resistance by the addition of 1 and 4% Mo,
Austenitic nickel alloys with resistance to concentrated (oxidizing) sulfuric acid require
high chromium, such as the ThyssenKrupp VDM alloy 33, or silicon, as in Haynes᭨
alloy D-205, and the stainless grades A610, A611, and Sandvik᭨
There are a few highly corrosion resistant nickel alloys with little or no chromium,
including the various Ni–Mo ‘‘B’’ grades and the 67Ni–31Cu alloy 400. Excellent in reduc-
ing environments, they have almost no tolerance to oxidizing compounds in the environment.
A newly developed nickel–molybdenum alloy, B-10, includes 8% Cr in its composition for
limited resistance to low levels of oxidizers.
Molybdenum, in contrast to chromium, has very low resistance to oxidizing solutions
but does resist reducing and halogen acids. Oxidizing acids such as nitric, aqua regia, and
concentrated sulfuric acids readily dissolve molybdenum metal. Hydroﬂuoric acid does not
affect Mo, and hot (110ЊC) hydrochloric acid attacks molybdenum metal only slowly.1
both stainless steels and nickel-base alloys, molybdenum as an alloying element is required
1 Effect of Alloying Elements 41
for resistance to halogen acids and to pitting by acid or oxidizing chlorides. The amount
used ranges from 2% in 316L stainless steel up to 24–30% in alloys B through B-10. As
an alloying addition, molybdenum improves the stability of the passive layer in the presence
Tungsten at the 2–4% level is used, along with molybdenum, to improve chloride pitting
Nickel metal in general is attacked by oxidizing solutions, while reducing solutions are
less aggressive. Some examples1
Temperature Corrosion Rate
Acid Notes (%) ЊC ЊF mm/yr mils/yr
Hydrochloric Air saturated 10 30 86 2 80
N2 saturated 10 30 86 0.25 10
Sulfuric Aeration 10 77 170 0.31 12.1
Air saturated 10 82 180 4 160
Nickel metal is strongly attacked by phosphoric acid solutions containing ferric (oxi-
dizing) salts, whereas it resists phosphoric acid solutions that are free of oxidizing com-
pounds. Nickel metal resists neutral chloride solutions, such as sodium chloride, but is
attacked by acid or oxidizing chloride salts. Alloys for use in reducing acids invariably have
a considerable nickel content, ranging from as little as 8% in 304L to as much as 71% in
Copper is generally resistant to reducing acid solutions containing only low levels of
oxygen but is readily attacked by oxidizing acids. These include nitric, sulfurous, and con-
centrated sulfuric acids as well as solutions containing oxidizing salts, such as ferric chloride.
Copper in solution tends to reduce the corrosion rate of stainless alloys in (reducing) sulfuric
acid. Those alloys intended for use in environments containing much sulfuric acid invariably
have some copper as an alloy addition. These include 904L, 20Cb-3᭨
, 825, Nicrofer᭨
hMo (alloy 31), and the Hastelloy᭨
alloys G, G-3, and G-30.
Additions of some 4 or 5% silicon increase resistance to corrosion in oxidizing envi-
ronments. The silicon is primarily used in alloys meant to withstand concentrated, hence
oxidizing, sulfuric acid. Such alloys in current production include A610, A611, Sandvik SX,
and Haynes D-205TM
. The use of silicon as an alloying element for corrosion resistance dates
back to before World War I. Although not a stainless steel, one of the oldest and most
generally corrosion resistant alloys ever developed is the 14.5% silicon cast iron, Duriron᭨
A silicon oxide ﬁlm is believed responsible for this grade’s useful resistance to environments
ranging from oxidizing to reducing. This includes seawater, and organic and many inorganic
acids, though not halogen acids. A further addition of 3% molybdenum provides resistance
to hot hydrochloric acid. Lack of strength and ductility limit the cast iron’s range of use.
When one speaks about the effect of this or that pure chemical on an alloy, one must
emphasize that real industrial environments are complex mixtures of chemicals. These
mixtures may behave in surprising ways, quite unlike what one might expect from the be-
havior of alloys in pure, laboratory-controlled environments. Corrosion rates depend not only
upon the concentrations of various chemicals but also on the temperature. The temperature
of liquid inside a vessel is one point that can be measured, but the temperature at the surface
42 Stainless Steels
of submerged heating coils in that vessel is another and higher value. Likewise the concen-
tration of, say, an acid in the vessel is not the same as the concentration at the point where
that acid is introduced to the mixture.
The most commonly used corrosion-resistant alloys are the stainless steels 304 (18%
Cr–8% Ni, commonly known as 18-8 stainless steel) and 316 (17% Cr–11% Ni–2% Mo).
The more corrosion resistant nickel alloys, such as C-276, have much higher levels of nickel,
57%, and molybdenum, 15.5%. Commercially pure nickel and nickel–copper alloys are used
for special environments.
Oxidizing and reducing environments are deﬁned chemically with respect to whether
hydrogen is oxidized or reduced under the environment in question. In an oxidizing envi-
ronment, hydrogen will only be present chemically combined with some other element, for
example with oxygen to form H2O. In a reducing environment that Hϩ
will be reduced to
hydrogen gas, H2.
Common oxidizing chemicals are nitric acid, HNO3, and certain salts such as ferric
chloride, FeCl3, and cupric chloride, CuCl2. The ferric and cupric ions are at relatively high
valences, ϩ3 and ϩ2, respectively, and readily accept electrons from, or oxidize, other ma-
terials to get their own valences reduced to a more stable level. Sulfuric acid, H2SO4, is
normally a reducing acid. At high concentrations, above about 95%, sulfuric acid changes
its character and becomes an oxidizing acid. Of course, dissolved oxygen contributes to the
oxidizing character of an environment. To some extent so does dissolved elemental sulfur.
To resist oxidizing conditions, an alloy must contain some amount of chromium. In an
oxidizing acid, simple materials such as 304 (18% Cr–8% Ni) or 310 (25% Cr–20% Ni) are
often used. An unusually high level of chromium, 33%, is present in a newly developed
alloy, UNS R20033, meant to resist very oxidizing acids. In any of these alloys the nickel
content is necessary to make a stable austenitic alloy, but it does not contribute speciﬁcally
to oxidizing acid resistance. Small additions of molybdenum or copper may be tolerated in
these alloys to enhance resistance to chlorides or sulfuric acid. But neither Mo nor Cu is
helpful in resisting strongly oxidizing chemicals.
A common and severe test for resistance to oxidizing acids is boiling 65% nitric acid.
The test is run for ﬁve periods of 48 h each, specimens being weighed after each test period,
and the results averaged. This test is a good measure of resistance to intergranular corrosion
in a sensitized alloy as well as to general corrosion in nitric acid. Test results2
at 0.13–0.20 mm/yr, which is good; 304 at 0.23 mm/yr; and RA333᭨
, which has been
stabilize annealed at 1700ЊF, at 0.29 mm/yr. In the case of RA333 it is the high chromium
that helps, in spite of the 3% Mo. Other molybdenum-bearing grades do not fare so well, at
316L (2% Mo) at 0.87 mm/yr after only 24 h, AL-6XN᭨
(6.3% Mo) at 0.74 mm/yr, 625
(9% Mo) at 0.76 mm/yr, and C-276 (15.5% Mo) at 0.74 mm/yr. These results do not mean
that one cannot successfully use a higher Mo alloy in the presence of any nitric acid at all.
They do indicate that high molybdenum alloys may not behave at all well in hot, concentrated
oxidizing industrial environments.
One cannot readily ﬁnd boiling 65% nitric acid (ASTM A 262 C) data for the 66% Ni–
31% Cu alloy 400 (Monel᭨
400) or for the assorted B alloys—B, B-2, B-3, or B-4. Their
corrosion rates in nitric acid are simply too high for the test to have any practical value.
Alloys 400, B, and B-2 have no deliberate chromium addition, B-3 and B-4 only about 1.3%
Cr. These grades may have excellent resistance to various reducing environments, but because
there is essentially no chromium present, they will literally dissolve in nitric acid. Likewise,
they are attacked by ferric, cupric and chlorate ions and even dissolved oxygen in HCl.
The common ‘‘reducing’’ acids are sulfuric under about 95%, phosphoric (H3PO4), and
hydrochloric. Of these by far the most corrosive is HCl, phosphoric being the less trouble-
some. Because reducing industrial environments often do contain some oxidizing salts or
2 Some Forms of Corrosion 43
oxygen from the air, most alloys used to withstand reducing chemical environments will
contain chromium, at least 15%. The alloy additions used to resist the reducing components
of the environment are nickel (Ni), molybdenum (Mo), and copper (Cu).
In sulfuric acid some amount of copper is usually used, such as in 20Cb-3᭨
steel, 904L, or 825. Even copper salts in the acid will reduce corrosion attack on stainless
steel. 20Cb-3 uses carefully balanced proportions of Cu and Mo to resist sulfuric acid cor-
2 SOME FORMS OF CORROSION
2.1 General Corrosion
This is the most common form of corrosion, accounting for the greatest tonnage loss of
metal. It is characterized by relatively uniform attack of the entire area exposed to the
corrosive environment. The passive ﬁlm slowly dissolves but continually re-forms. Since the
attack is linear with time, the life of equipment subject to general corrosion is reasonably
predictable. If the passive ﬁlm is locally disrupted, as by chlorides, corrosion modes such
as pitting, crevice, and stress corrosion may occur. These are more difﬁcult to predict and
tend to cause premature equipment failures. Erosion may also remove the passive ﬁlm and
contribute to much higher than expected general corrosion rates.
Stainless steel passivates simply by being exposed to air. A metallographic specimen of
AL-6XN, for example, must be etched immediately after polishing. Otherwise it will pas-
sivate in air so that a uniform etch cannot be achieved. Passivation in acid is not required.
But, during normal fabrication practices, enough iron is picked up to cause surface rusting
in damp weather. A treatment in nitric–hydroﬂuoric acid may be used to remove this surface
Uniform corrosion rates may be stated as an average metal thickness loss with time, in
mils per year or millimeters per year. A convenient rating for metals subject to uniform
attack based on corrosion rates is as follows:
Excellent—rate less than 5 mils/year (0.13 mm/yr). Metals suitable for making critical
Satisfactory—rate 5–50 mils/yr (0.13–1.3 mm/yr). Metals generally suitable for non-
critical parts where a higher rate of attack can be tolerated
Unsatisfactory—rates over 50 mils/yr (1.3 mm/yr). Metals usually not acceptable in
An approximate ranking of a few common alloys by increasing resistance to general cor-
rosion would be 304L, 316L, 2205, 20Cb-3/825, RA333, AL-6XN, 625, and C-276. Alloy
selection does depend upon the exact corrosive environment in question. Some speciﬁc ex-
amples include hot concentrated caustic, where commercially pure nickel or the 76% nickel
alloy 600 is used. Alloy 33 may be required for mixtures of caustic with oxidizing chemicals.
For sulfuric acid alloys 20Cb-3 or 825 are usually chosen; however, if chlorides are present
in the acid, one of the 6% molybdenum grades such as AL-6XN would be preferred. AL-
6XN is used for organic acids, such as napthenic acid in reﬁnery service. For nitric acid
service chromium is beneﬁcial, molybdenum not. Alloys commonly selected include 304L
or a low-carbon version of 310. RA333 is used when the same piece of equipment must see
very high temperatures, in the red heat range, in one zone and aqueous corrosion in another.
44 Stainless Steels
2.2 Stress–Corrosion Cracking
For just about every alloy, there is some chemical environment that, combined with stress,
will cause cracking. For brass that environment is ammonia or other nitrogen compounds.
The source of stress is usually residual forming and welding stresses, which may reach the
yield point of the material. Operating stress is rarely the issue.
For austenitic stainless steels chlorides are the major cause of stress–corrosion cracking
(SCC). An example is hot potable water under heat transfer conditions which permit chlo-
rides to concentrate locally. Susceptible alloys include 304L, 316L, 321, and 347. Some 95%
of 316L chemical plant equipment failures may be attributed to chloride SCC. The chlorides
concentrate from trace amounts present in steam for heating or the cooling water in heat
exchangers as well as from the product
Chloride SCC occurs most quickly in austenitic stainless steels with about 8–10% nickel,
alloys with much lower or much higher nickel content being less susceptible. As thermal
stress relief is rarely practical with stainless fabrications, the metallurgical solution is a
change in alloy. Nickel-free ferritic steels, such as E-BRITE, are highly resistant to chloride
SCC but impractical to fabricate into a vessel.
The traditional solution in North America has been to go to a higher nickel alloy. Alloys
with about 30% or more nickel are generally considered to be good engineering solutions
to most chloride SCC problems, although they will crack under very severe conditions. 20Cb-
3 at about 34% and 825 at 40% nickel have long been chosen for this service. Likewise the
800, UNS N08800, 31% Ni, had been used in years past. However,
this low-carbon, ﬁne-grained version of 800 is now rarely available. Regardless of what it
is called, ‘‘800’’ today usually is 800HT᭨
, UNS N08811, a higher carbon, coarse-grained
version. This grade is designed to maximize creep rupture strength for high-temperature
Since the mid-1980s the 6% molybdenum superaustenitics have become available.
Grades such as 254 SMO᭨
with only 18% nickel, or AL-6XN at 24% nickel, have been
used effectively to resist chloride SCC. The material cost of the ‘‘6-moly’’ grades is between
that of 316L stainless and nickel alloy C-276. Although lower in nickel, molybdenum con-
tents above 2% tend to decrease susceptibility of austenitic stainless steel to chloride SCC.3
For greater resistance to both corrosion and chloride SCC the most used grade has been
C-276, at 57% Ni 15.5% Mo. There are now a number of alloys in this class, including C-
686, C-2000, 59, and a new Japanese grade, MAT 21. These very high nickel
alloys can easily reach ﬁve times or more the cost of 316L stainless steel. They are metal-
lurgically excellent solutions to chloride SCC, particularly in severe environments. However,
they are expensive choices for service conditions under which 316L lasted a few years before
cracking. There is a less expensive choice, one that has long been used in Europe—a duplex
stainless steel which is about half austenite and half ferrite. Duplex stainless steel is a prac-
tical solution to most 304L or 316L SCC failures. The most commonly available duplex in
North America is 2205, at a cost roughly 20% above that of 316L.
Other forms of SCC in stainless steels include caustic cracking and polythionic acid
SCC. Caustic may crack carbon as well as stainless steel. High-nickel alloys, such as al-
loy 600 or, better, commercially pure nickel (UNS N02201), are used for hot concentrated
Polythionic acid stress–corrosion cracking (PASCC) is caused by sulfur compounds in
the environment and most often encountered in reﬁneries. Any stainless or nickel alloy that
has been sensitized can be subject to PASCC. High-nickel alloys do not help; even 600 alloy
will crack when sensitized.4
To resist this form of SCC the alloy must contain a strong
carbide-forming element, or ‘‘stabilizing’’ element, such as columbium or titanium. Examples
2 Some Forms of Corrosion 45
include 321, 347, 20Cb-3, 825, and 625. In addition, the alloy must be given a stabilizing
anneal so that the carbon is effectively combined with the Cb or Ti. RA333, because of its
tungsten and molybdenum content, resists PASCC when stabilize annealed about an hour at
Normally, 304H or 316H would be quite sensitive to polythionic acid stress cracking,
as these higher carbon, solution-annealed alloys readily sensitize. The matter has been ad-
dressed at one reﬁnery by fabricating the equipment from one of these H-grade stainless
steels, then stabilize annealing the completed fabrication. A temperature of about 1650ЊF
(900ЊC) for a minimum of 1 h is used. This does precipitate carbides at the grain boundaries,
but the temperature is high enough to permit chromium to diffuse back into the Cr-depleted
grain boundary zone. In addition, this treatment relieves over half of the residual fabricating
stress, thus reducing susceptibility to chloride SCC as well.
2.3 Pitting Corrosion
Pitting is an extremely localized form of corrosion that results in holes in the metal. Although
total metal loss may be small, the equipment may be rendered useless because of perforation.
Pitting usually requires a long initiation period before attack is visible. Once a pit has begun,
the attack continues at an accelerating rate. Pits tend to grow in a manner that undermines
or undercuts the surface. Typically a very small hole is seen on the surface. Poking at this
hole with a sharp instrument may reveal a rather cavernous hole under what had looked like
solid metal. In effect, a pit may be considered a self-formed crevice. Pitting attack increases
Chloride solutions are the most common cause of pitting attack on stainless steels and
nickel alloys. The alloying additions molybdenum, nitrogen, and, to some extent, chromium
all contribute to pitting resistance. A laboratory measure of resistance to pitting corrosion is
the critical pitting temperature, or CPT, which is the highest temperature at which an alloy
resists pitting in a given environment. Alloy ranking with respect to chloride pitting resistance
would be 304L (0% Mo, poor), followed by 316L (2% Mo), then four austenitics each with
about 3% molybdenum, 20Cb-3/825/317L/RA333, the duplex 2205 (3% Mo–0.16% N),
AL-6XN (6.3% Mo–0.22% N), 625 (9% Mo) and C-276 (15.5% Mo). Alloys AL-6XN and
higher have sufﬁcient chloride resistance to be used in hot seawater service. The lower
molybdenum grades, including 2205 with 3% Mo, are unsuitable for use in seawater.
2.4 Crevice Corrosion
Crevice corrosion, more so than pitting, is the limiting condition which often prevents the
use of conventional austenitic stainless steel in chloride environments. The attack usually
occurs in small volumes of stagnant solution under gasket surfaces, lap joints, marine fouling,
and solid deposits and in the crevices under bolt heads and the mating surfaces of male and
female threads. The mechanism involves oxygen depletion in the crevice followed by chlo-
ride ion concentration and increase in acidity (decrease in pH) within the crevice. In a neutral,
pH 7, chloride solution service the liquid within a crevice may contain 3–10 times as much
chloride as the bulk solution and have a pH of only 2–3.
Susceptibility to crevice corrosion increases rapidly with temperature. Molybdenum and
nitrogen additions to nickel–chromium–iron alloys improve their resistance to crevice cor-
rosion. Together with the use of appropriate materials, design practice to minimize crevices
and maintenance procedures to keep surfaces clean are required to combat the problem.
46 Stainless Steels
The usual laboratory measure of resistance to crevice corrosion is the critical crevice
corrosion temperature, or CCCT, which is the highest temperature at which an alloy resists
crevice corrosion in a given environment. For a given environment the CCCT is usually
signiﬁcantly lower than the CPT. Crevice corrosion resistance as measured by the ferric
chloride test relates, to a degree, to performance in seawater. The results for a number of
given the temperature for initiation of crevice corrosion in 10% ferric chloride (FeCl3
⅐6H2O) per ASTM G 48 Practice B and pitting reseistance equivalent (PRE) N ϭ Cr ϭ 3.3%
Mo ϩ 30(%N) are as follows:
Alloy (%) ЊC ЊF Equivalent, N Reference
316L 2.1 Ϫ3 27 23 5
825 2.7 Ϫ3 27 30 5
317L 3.2 2 35 29 5
2205 3.1 20 68 38 5
4.4 20 68 34 5
28 3.5 24 75 38 6
904L 4.4 24 75 35 5
904L 4.4 25 77 35 7
G 6.5 30 86 43 5
28 3.5 35 95 39 7
2507 4.0 35 95 47 7
1925hMo 6.2 40 104 47 7
33 1.4 40 104 50 7
AL-6XN 6.2 43 110 48 5
27-7MO 7.3 45 113 57 8
625 9.0 45 113 51 5
625 9.0 55 131 51 6
31 6.5 55 131 54 6
G-30 5.5 50 122 48 7
C-276 15.4 55 130 66 5
2.5 Intergranular Corrosion
Intergranular corrosion consists of localized attack along the grain boundaries of the metal.
Sensitization to this attack in stainless or nickel alloys is caused by precipitation of
chromium-rich carbides in the grain boundaries at a temperature low enough that a
chromium-depleted zone forms. This precipitation most commonly occurs from the heat of
welding. It may also result from a slow cool after annealing or from prolonged exposure to
intermediate temperatures, roughly 850–1470ЊF (450–800ЊC), in service.
A most effective means of combating intergranular corrosion is to restrict the carbon
content of the alloy. In the stainless ‘‘L’’ grades 0.03% maximum is considered sufﬁcient.
High chromium and molybdenum additions, as in AL-6XN, also reduce the chance of in-
Another approach is to add columbium or titanium to tie up the carbon, the same as is
done to resist PASCC. 20Cb-3 stainless steel takes both approaches, being melted to low
carbon as well as having a columbium addition.
3 AOD, Dual Certiﬁcation, and Chemistry Control 47
2.6 Galvanic Corrosion
An electrical potential, or voltage, difference usually exists between two different metals that
are in electrical contact and immersed in a corrosive solution. This potential difference causes
current to ﬂow and the less noble, or more anodic, metal suffers increased corrosion rate.
The severity of attack depends upon the relative voltage difference between the metals, the
relative exposed areas of each, and the particular corrosive environment.
The most common example is the old-fashioned ﬂashlight battery, or dry cell. It has a
shell of zinc metal (less noble, or anodic) ﬁlled with a moist corrosive paste that conducts
electricity. The center post is made of graphite, which is quite noble (cathodic, does not tend
to corrode). The potential (voltage) difference between zinc and graphite is about 1.5 V.
When an electric connection is made in a ﬂashlight, the zinc corrodes, giving up electrons,
which ﬂow through the lightbulb toward the graphite cathode, the positive pole. In this
case, because generating electricity is the point, no one minds that the zinc corrodes and
gets used up.
The ratio of cathodic (noble) to anodic areas is an important factor in galvanic corrosion.
An undesirable situation is a large cathode connected to a small anode, or less noble metal.
This can develop high current density, hence severe corrosion, at the anode. In that common
zinc dry cell the zinc anode has a much larger area than the graphite cathode, so it has some
useful working life before corroding through the zinc case.
For example, a large area of stainless steel in contact with a small surface area of carbon
steel is undesirable. The potential difference will tend to corrode the carbon steel, and the
very large area of stainless steel will make that corrosion occur quickly. The reverse condition
is preferred. That is, a small area of stainless (or more noble) metal may be coupled with a
much larger area of carbon steel (anodic) without signiﬁcant problems. ‘‘Signiﬁcant’’depends
upon the application. In the past, when ferritic stainless trim was used on carbon steel
automobile bodies, the steel would tend to corrode most severely underneath the trim. In
part that was because the crevice trapped salt, but it was accentuated by the galvanic differ-
ence between ferritic stainless and carbon steel.
There is some potential difference among the various stainless and nickel alloys. In
practice, galvanic corrosion is rarely a problem among these various alloys. There is, how-
ever, a signiﬁcant potential difference between copper and stainless alloys. So long as the
stainless steel is passive (not actively corroding), it is more noble enough than copper to
corrode the copper alloy. An example is when a heat exchanger with a Muntz metal (60%
Cu–40% Zn) tubesheet is retubed with AL-6XN᭨
alloy instead of the original copper–nickel
tubes. The potential difference is enough to corrode the copper alloy tubesheet. One ought
to either replace the tubesheet with stainless steel, or retube using a copper-base alloy.
Graphite is at the noble end of the galvanic series. If graphite is in contact with stainless
or nickel alloys in a corrosive environment, those alloys may corrode preferentially.
Galvanic effects have a positive side and may be used to protect equipment from cor-
rosion, a common example being a zinc coating on steel. The zinc corrodes preferentially,
and in doing so protects the steel from corrosion (rusting). Zinc or magnesium anodes are
often connected to equipment ranging from chemical process to steel ship hulls to protect
them from corrosion.
3 AOD, DUAL CERTIFICATION, AND CHEMISTRY CONTROL
Most stainless steels, and a few higher nickel alloys, are available with different levels of
carbon. For resistance to intergranular corrosion, a low carbon is preferred, usually 0.03%
48 Stainless Steels
carbon maximum in stainless steel. This is referred to as an ‘‘L’’ grade stainless steel, e.g.,
304L and 316L. With respect to aqueous corrosion resistance, the lower the carbon, the
better. For high-temperature service the opposite is true, and some minimum amount of
carbon is required for both tensile and creep rupture strength.
The argon-oxygen decarburization (AOD) process for reﬁning stainless steel was intro-
duced in the 1970s. This made profound changes in how existing grades were produced as
well as permitting totally new grades to be developed. Three of these changes are worth
discussing—carbon, sulfur, and precise control of chemistry.
Prior to the AOD, carbon could not be removed in the reﬁning process without also
removing chromium. Low-carbon grades could only be produced by starting with low-carbon
raw materials, speciﬁcally low-carbon ferrochrome. The expense of low-carbon ferrochrome
meant that the L grades were inherently more expensive. The AOD now permits reﬁning
carbon to very low levels, even with starting stock of higher carbon.
Industrywide speciﬁcations such as the American Society for Testing and Materials
(ASTM) were written prior to the introduction of this new melting process. For example,
ASTM A 240 for 304 stainless steel, UNS S30400, calls out 0.08% carbon maximum, no
minimum, 30,000 psi minimum yield strength. Low carbon 18-8, 304L, S30403 is limited
to 0.03% carbon, with a consequent lower limit for yield strength, 25,000 psi minimum. In
addition, there is a 304H, meant for high-temperature use, with carbon speciﬁed as a range,
0.04–0.10%, and annealing and grain size requirements. This constitutes three separate
grades. It is more economical if the mills can melt steel to only two, not three, different
levels of carbon and dual certify. Consider 304, UNS S30400. As the carbon is speciﬁed
only as a maximum, it might be possible to melt 304 to 0.03 maximum carbon. Lower
carbon would also result in lower than the 30,000 psi yield strength required. However, using
the AOD it is now possible to add a very small, precisely controlled amount of nitrogen.
This does not harm intergranular corrosion resistance, but it does tend to increase room
temperature tensile properties. With care in annealing practice, it is possible to produce 304
with low enough carbon to meet the 304L speciﬁcation yet with high enough yield strength
to meet 304 requirements. As this metal meets all speciﬁed requirements of both 304L and
304, the mill test report will show both S30403 and S30400, i.e., dual certiﬁed.
S30403/S30400 is appropriate for corrosion service but not for high-temperature me-
chanical properties. For useful creep rupture strength some minimum amount of carbon is
required, typically 0.04%. The situation was addressed a few years ago by adding a number
of H grades to ASTM A 240, with controlled carbon for high-temperature strength. The
stainless steel 304H, S30409 has carbon speciﬁed at 0.04–0.10% for high-temperature
strength. In addition, there are grain size and minimum anneal temperature requirements.
The 304, S30400 has no requirement for minimum carbon, control of grain size, or annealing
temperature. Therefore any 304H containing no more than 0.08% carbon will meet 304
requirements and may be dual-certiﬁed with 304. One should note that dual-certiﬁed
304L/304 is suited only for aqueous corrosion service but would have rather low strength
at high temperature. Likewise dual-certiﬁed 304/304H is meant for high-temperature service
but may be unsatisfactory for welded construction in a wet corrosive environment. In prac-
tice, there is rather little actual S30400 produced as sheet or plate at this time. Most is dual
certiﬁed, one way or another.
Like carbon, sulfur can now readily be reﬁned to very low levels, typically less than
0.005%. Compare this with typical ASTM A 240 levels of 0.030% S maximum. Usually,
stainless steel intended for plates is reﬁned to a low-sulfur level to improve hot workability.
The plate is generally formed and welded, with little machining by the customer. Low sulfur
is quite detrimental to machinability. As bar products are commonly meant to be machined,
most stainless bar actually must be resulfurized to some level, about 0.02%, for improved
machinability. When a plate is intended to be drilled for a tubesheet, machinability becomes
5 Ferritic Stainless Steel 49
important and a resulfurized grade, still within the old 0.030 sulfur maximum, may be
It is the precise control of chemistry, in particular nitrogen, that has permitted devel-
opment of the superaustenitic 6% molybdenum grades. The ability to closely control nitrogen
as an alloying addition has also tremendously improved the weldability of duplex stainless
steels. Whereas formerly the only duplex stainless steel used in North America was 3RE60,
and that only in tubing, today several grades of duplex stainless plate, pipe, and bar products
are used in signiﬁcant and growing amounts.
Chemistry control also means that the producer will minimize the use of expensive
alloying elements. To remain competitive, mills now melt to the bottom end of the allowable
range. One consequence for the user is that 316L, speciﬁed as 2.00–3.00% Moly, now has
a melt range of about 2.00–2.10% Mo. Through the 1970s the typical Mo level of 316L
was about 2.3%. In addition, the average nickel content has dropped from just below 12%
in the 1970s down to around 10.2% Ni as currently produced. The result has occasionally
been that 25-yr-old 316L equipment, replaced in kind, gave unexpectedly short life. In part,
of course, this is due to increased corrosive conditions from recycling, rather than dumping,
The metallurgical aspects of alloy selection are well covered in this and other works. Along
with corrosion resistance, strength, and fabricability, one of the most important material
properties is availability. On a large project most alloys can be made in all product forms,
in full mill heat lots. A contemporary example is 317LMX᭨
, used as ﬂat-rolled product in
mill heat lot quantities for ﬂue gas desulfurization scrubbers. This grade is rarely, if ever,
carried in stock by mills or service centers.
Few mills produce all the forms, such as sheet, plate, bar, pipe, pipe ﬁttings, and ap-
propriate weld ﬁllers, needed to fabricate a chemical process vessel. The minimum quantity
a mill requires per product form is large, and lead times can be signiﬁcant. This may limit
ﬂexibility in the event of error, last-minute design changes, or later maintenance needs.
Consider what alternate, if more expensive, grade may be used to ﬁll in for unavailable
product forms or sizes. For example, AL-6XN has occasionally been used to ﬁll out a bill
of materials speciﬁed 317LMX. The stainless steel grades 304L and 316L are used in such
quantity that availability is unlikely to be an issue. The same may not be true for more
highly alloyed or specialized materials.
5 FERRITIC STAINLESS STEEL
The ferritic grades listed below exhibit corrosion resistance over a very wide range. All are
subject to severe embrittlement after prolonged exposure in the 700–1100ЊF (370–600ЊC)
temperature range. Alloy 409 is weldable and is the alloy used for automotive exhaust
systems and catalytic converter shells. It has some useful high-temperature oxidation resis-
tance to about 1200ЊF (650ЊC). In plate gauges it may be welded with ERNiCr-3 for better
toughness. Alloy 409 is not suited for decorative applications as it may rust from exposure
to weather. Alloy 416 is free machining, available both as a ferritic and a martensitic version;
430 is commonly used for decorative purposes as well as food-handling equipment. E-BRITE
has chloride-pitting resistance equal or superior to 316L and practical immunity to chloride
SCC. E-BRITE is currently available only as tubing for heat exchangers. AL29-4-C᭨
extremely resistant to chloride pitting and is used for heat exchanger applications, available
only as tubing or thin strip.
50 Stainless Steels
Cr Ni Mo Si Mn Cu C Fe Other
409 S40900 11 — — 0.4 0.3 — 0.015 87 —
405 S40500 12 — — 0.3 0.5 — 0.06 86 0.3 Al
416 S41600 13 — — 0.5 1 — 0.05 85 0.2 S, 0.04 P
430 S43000 16.5 — — 0.5 0.5 — 0.08 83 —
439 S43035 17.2 — — 0.5 0.4 — 0.015 81 0.5 Ti
S44627 26 — 1 0.2 0.1 — 0.002 72 0.1 Cb
S44735 29 — 4 0.35 0.3 — 0.02 66 0.5 Ti
6 MARTENSITIC STAINLESS STEELS
The only one of these that is readily welded is 410S. The higher carbon 410 may require
signiﬁcant preheat and postweld anneal. Consider the nickel alloy ﬁller ERNiCr-3 for max-
imum resistance to weldment cracking at a sacriﬁce in strength and hardness. The corrosion
resistance of 410 depends upon the heat-treated condition. For maximum corrosion resistance
temper either below 750ЊF (400ЊC) or above 1100ЊF (600ЊC). Both the 410 and the marten-
sitic 416 are used in sporting arms construction. The 440 series are used for cutting tools,
440A and B for pocket knives; 440C and 154CM have the best edge retention and are used
for ﬁne custom knives and surgical tools.
Cr Ni Mo Si Mn C Fe Other
410 S41000 12 — — 0.3 0.4 0.14 87 —
410S S41008 12 — — 0.3 0.4 0.05 97 —
416 S41610 13 — — 0.4 0.2 0.1 84 0.2 S, 0.05 P
420 S42000 13 — — 0.4 0.4 0.2 86 —
431 S43100 15.6 1.9 — 0.2 0.4 0.1 81 —
440A S44002 17 — 0.5 0.2 0.4 0.67 81 —
440B S44003 17 — 0.5 0.2 0.4 0.8 81 —
440C S44004 17 — 0.5 0.2 0.4 1.07 80 —
— 14 — 4 0.3 0.5 1.05 80 —
7 AGE-HARDENING MARTENSITIC STAINLESS STEELS
Cr Ni Mo Cu Mn Al Ti C Fe Other
455 S45500 11.5 8.5 — 2 0.2 — 1.1 0.2 76 0.3 Cb
S15700 15 7 2.5 — 0.4 1 — 0.04 74 —
S17400 15.5 4.7 — 3.3 0.5 — — 0.05 75 0.3 Cb
S17780 17 7.3 — — 0.7 1.2 — 0.06 74 —
S13800 23 8 2.5 — — 1.2 — 0.03 76 —
9 Austenitic Stainless and Nickel Alloys 51
8 DUPLEX STAINLESS STEELS
Duplex stainless steels are characterized by high strength and good resistance to chloride
SCC. They represent a more economical solution to the problem of stainless SCC than does
the use of a high-nickel alloy. Some of the newer lean duplex grades, such as LDX 2101,
are replacing carbon steels as well as 304L and 316L stainless steel. AL 2003 is intended
to offer a cost reduction compared with 2205. Carbon steel may be replaced in part because
the higher strength permits such weight reduction as well as eliminating maintenance costs.
The grades most commonly available from North American service centers are alloys 2205
and 255. LDX 2101 is beginning to be used in Europe. Other grades are available from steel
mills in heat lot quantities, appropriate for large projects.
Cr Ni Mo Cu Mn Si N C Fe Other
S32101 21.5 1.5 0.3 0.3 5 0.7 0.22 0.03 70 —
S32003 21 3.5 1.6 — 1 0.5 0.17 0.02 73 —
SAF 2304 S32304 23 4 0.3 0.3 2 — 0.1 0.03 70 —
3RE60 S31500 18.4 4.8 2.7 — 1.6 1.7 0.07 0.03 70 —
19D S32001 21.2 1.3 — — 5 0.4 0.15 0.02 71 —
2205 S32205 22.1 5.6 3.1 — 1.5 0.5 0.16 0.02 67 —
100 S32760 25 7 3.5 0.5 0.5 0.3 0.22 0.02 62 0.7 W
2507 S32750 25 7 4 — 0.1 0.2 0.3 0.02 63 —
329 S32900 26.5 4.2 1.5 — 1 0.8 — 0.08 66 —
S32950 26.5 4.8 1.5 — 0.4 0.3 0.2 0.02 66 —
255 S32550 25.5 5.7 3.1 1.8 0.8 0.5 0.17 0.02 62 —
9 AUSTENITIC STAINLESS AND NICKEL ALLOYS
These nickel-bearing alloys are used for the majority of corrosive environments. Alloy 316L
is by far the most common choice for chemical process equipment. Formerly, when 316L
was inadequate, the designer switched to the high end of the spectrum, alloy C-276, which
is still considered the most broadly useful of the high-nickel alloys. Today there are numerous
other choices, ranging from those of intermediate cost to alloys superior to C-276 in speciﬁc
Types S30600, S32615, and alloy D-205TM
are specialized high-silicon materials in-
tended for concentrated sulfuric acid heat exchanger service. Weldability is limited. A very
high chromium grade, R20033, is also intended for hot concentrated sulfuric acid. It is
weldable and has a broader range of potential uses than do the high-silicon alloys.
Materials in the 5–7% molybdenum range are used for seawater service and chemical
process vessels in general. Alloys N08367, S31254, and N08926 constitute the ‘‘6 moly’’
alloys. These have both corrosion resistance and cost intermediate between 316L and alloy
C-276. All are readily fabricated and broadly available. Nitrogen in these alloys retards sigma
formation, in spite of rather high Mo and moderate Ni levels. Prolonged exposure in the
1000–1800ЊF (540–980ЊC) temperature range may cause sigma-phase precipitation.
Alloys in the 13–16% Mo range include C-276, C-22, 59, C-2000, and 686. The latter
four are regarded as improvements over C-276, with higher Cr for oxidizing environments.
52 Stainless Steels
The newest, and possibly best of the very high end nickel alloys, MAT 21, makes use of a
tantalum addition as well as 19% Mo.
Alloy selection for corrosive process environments is a complex process. It should in-
clude experience with similar equipment, extensive testing in the exact corrosive environment
of interest, and detailed knowledge of the various alloys to be considered. Oftentimes, ap-
parently minor contaminants can cause major changes in corrosion rates. One example is
contamination of organic chlorides with small amounts of water. This can permit the organic
compound to hydrolyze, forming hydrochloric acid. The HCl in turn may aggressively pit
or stress corrode the standard 18-8 stainless steels. Other examples include the alloys B-2,
200, and 400, which contain no chromium. While they have excellent corrosion resistance
in reducing environments, they have little or no resistance to oxidizing environments. Un-
expected failures may therefore arise from contamination by small amounts of oxidizing salts
(e.g., FeCl3, CuCl2, or NaClO3) or even dissolved oxygen. Titanium behaves in the opposite
manner and requires the presence of oxidizing species to develop its protective oxide ﬁlm.
Cr Ni Mo Si Mn Cu C Fe Other
302 S30200 18.5 8.2 — 0.5 0.75 — 0.1 72 —
304L S30403 18.3 9 — 9.5 1.7 — 0.02 70 —
321 S32100 17.3 9.3 — 0.7 1.8 — 0.01 70 0.2 Ti
347 S34700 17 9.5 — 0.7 1.5 — 0.04 70 0.5 Cb
316L S31603 16.4 10.2 2.1 0.5 1.6 — 0.02 69 —
317L S31703 18 11.6 3.1 0.4 1.5 — 0.02 65 —
317LMN S31726 17 13 4.2 9.5 1.5 — 0.03 62 0.15 N
A610 S30600 18 15 — 4 0.7 — 0.01 62 —
S31254 20 18 6.1 0.4 0.7 0.7 0.015 54 0.2 N
SX S32615 18 20.5 0.9 5.5 1.5 2 0.04 51 —
S32654 24 22 7.3 — 3 0.5 0.01 42 0.5 N
B66 S31266 24.5 22 5.6 — 3 1.5 0.02 44 2 W
904L N08904 21 25 4.5 0.5 1.7 1.6 0.015 45 —
1925 hMO, 25-6MO N08926 20 25 6.2 0.4 0.7 0.9 0.01 46 0.2 N
N08367 20.5 24 6.3 0.4 0.3 — 0.02 48 0.22 N
N08927 22 27 7.3 0.2 1 — 0.01 42 0.35 N
28 N08028 27 31 3.5 0.2 1.8 1 0.01 35 —
31 N08031 27 31 6.5 0.2 1 1.2 0.01 33 0.2 N
33 R20033 33 31 1.4 0.3 0.7 0.7 0.01 32 —
20Cb-3 N08020 20 33 2.2 0.4 0.4 3.3 0.02 40 0.5 Cb
3620 Nb N08020 20 37 2.1 0.5 1.6 3.4 0.02 35 0.6 Cb
825 N08825 21.5 40 2.8 0.3 0.6 2 0.01 29 0.8 Ti
N06333 25 45 3 1 1.5 — 0.05 18 3 Co, 3 W
G-30 N06030 29.5 45 5.5 — — 1.9 0.01 15 0.7 Cb, 2.5 W
G N06007 22 45 6.5 0.3 1.5 2 0.01 20 2.1 Cb, 0.8 W
G-3 N06985 22 48 7 0.4 0.8 2 0.01 18 0.3 Cb, 0.8 W
625 N06625 21.5 61 9 0.1 0.1 — 0.05 4 3.6 Cb
C-276 N10276 15.5 57 15.5 0.05 0.5 — 0.005 5.5 0.2 V,4 W
686 N06686 20.5 57 16.3 0.1 0.2 — 0.005 1 3.9 W, 0.2 Al
N06200 23 58.5 16 0.02 0.2 1.6 0.003 0.3 0.25 Al
C-22 N06022 21 57 13 0.05 0.3 — 0.003 4 0.2 V, 3 W
59 N06059 23 59 16 0.05 0.4 — 0.005 0.3 0.2 Al
MAT 21 — 19 60 19 — — — — — 1.8 Ta
10 Welding 53
Cr Ni Mo Si Mn Cu C Fe Other
D-205 — 20 64 2.5 5 — 2 0.02 6 —
B-2 N10665 — 71 28 0.01 0.15 — 0.002 0.8 —
B N10001 — 66 30 — 0.5 — 0.06 3 0.3 V
B-3 N10675 1.3 67.7 28 0.03 0.5 — 0.002 1.5 —
B-4 N10629 1.3 67 28 — — — 0.005 3 —
400 N04400 — 66 — 0.02 1 31 0.1 1.5 —
K500 N05500 — 66 — — 1 28 0.1 1.5 2.7 Al, 0.6 Ti
600 N06600 15.5 76 — 0.2 0.3 — 0.08 8 0.2 Ti
201 N02201 — 99.5 — 0.2 — — 0.01 0.2 —
Alloys listed in boldface are those most commonly available from stocking distributors.
There are some important differences between welding carbon steel and welding stainless
steel. Alloys containing more than about 20% nickel have somewhat different requirements
than the lower nickel austenitic stainless steels. There are speciﬁc issues regarding duplex
stainless steels and weld ﬁllers for the high-molybdenum grades.
10.1 Carbon versus Stainless Steel
Six important differences between welding the carbon or low-alloy structural steels and the
austenitic stainless and nickel alloys are surface preparation, shielding gases, cold cracking
versus hot cracking, distortion, penetration, and fabrication time.
1. Surface Preparation. When fabricating carbon steel, it is common practice to weld
right over the scale (a so-called mill ﬁnish is a layer of blue-black oxide, or scale, on the
metal surface), red rust, and even paint. The steel weld ﬁllers normally contain sufﬁcient
deoxidizing agents, such as manganese and silicon, to reduce these surface iron oxides back
to metallic iron. The resultant Mn–Si slag ﬂoats to the weld surface. Iron oxide, or scale,
melts at a lower temperature, 2500ЊF (1371ЊC), than does the steel itself. One can see this
in a steel mill when a large ingot is removed from the soaking pit for forging—the molten
scale literally drips off the white-hot steel
Stainless steel, by contrast, must be clean and free of any black scale from hot-rolling,
forging, or annealing operations. Such scale is predominately chromium oxide. Normally,
stainless steel is produced with a descaled white or bright ﬁnish. Stainless steel melts at a
lower temperature than does its chromium oxide scale, and the stainless steel weld ﬁller
chemistry is not capable of reducing this scale back to metallic chromium. As a result, with
gas shielded processes it is difﬁcult to get the weld bead to even ‘‘wet,’’ or stick to, a scaled
piece of stainless steel.
The need to clean or grind down to bright metal is more likely to cause trouble when
stainless steel is being joined to carbon steel. In this dissimilar metal joint it is necessary to
grind that carbon steel to bright metal, on both sides of the joint, free of all rust, mill scale,
grease, and paint. The preferred weld ﬁllers for this particular joint, to minimize the potential
for any hard martensitic layer on the steel side, are ENiCrFe-3 covered electrodes or ERNiCr-
3 bare ﬁller wire; E309 electrodes are commonly used but are not the optimum choice.
54 Stainless Steels
Both stainless and high-nickel alloys designed for corrosion resistance are produced to
very low carbon contents, less than 0.03% and sometimes less than 0.01% carbon. Any
higher carbon content will reduce the metal’s corrosion resistance. For this reason it is
necessary to clean the alloy thoroughly of all grease and oil before welding. Also the very
high nickel alloys, such as Monel᭨
400 or commercially pure nickel 200/201, are very
sensitive to weld cracking from the sulfur in oil or marking crayons.
Metallic zinc paint is a common way to protect structural steel from corrosion. Even a
small amount of that zinc paint overspray on stainless steel will cause it to crack badly when
welded. Consider ﬁnishing all stainless steel welding before painting the structural steel in
2. Shielding Gases. For gas–metal arc welding (GMAW, also called MIG) of the carbon
steel the shielding gases are usually 95% Ar–5% O, 75% Ar–25% CO2 (carbon dioxide), or
100% CO2. While suitable for carbon or low-alloy steel welding wire, such gases are far too
oxidizing for use with stainless or nickel alloys. It is not unknown to hear the complaint
‘‘Clouds of red smoke are coming off when I weld this stainless. . .heavy spatter’’ and then
learn that the shielding gas used was 75% Ar–25% CO2—a ﬁne gas for carbon steel but not
for any stainless steel.
One exception to this high CO2 prohibition is when using ﬂux-cored wire, either stain-
less or nickel alloy. Some of these wires are speciﬁcally formulated to run best with 75%
Stainless and nickel alloys may be GMAW spray-arc welded using 100% argon shielding
gas, though it is not necessarily the ideal choice. Stainless steels possess a passive chromium
oxide ﬁlm. The basis of stainless steel corrosion resistance, this ﬁlm is not desirable when
welding. Some 80% argon is necessary to get into a spray transfer mode. Beyond this, a
helium addition, up to about 20%, gives a hotter arc and helps break up the oxide ﬁlm. A
very slight amount of CO2, perhaps 1%, will prevent arc wander. Too much CO2 may begin
to add carbon to the weld, undesirable for corrosion resistance. Nitrogen may be added in
gases speciﬁcally designed for welding the duplex stainless steels.
Pulse-arc welding is usually done with a 75% Ar–25% He mix. Short-circuiting arc
transfer may be done with this 75% Ar–25% He mix but a 90% He–7 % Ar–2 CO2
– –%2 2
‘‘trimix’’ is more commonly used.
3. Cold Cracking versus Hot Cracking. Carbon steel weldments may harden and crack
as they cool from welding. High hardness and the resulting cracking may occur when the
steel contains more than 0.25% carbon. Alloying elements which increase hardenability, such
as manganese, chromium, molybdenum, etc., can make steels of lower carbon content also
harden. Hydrogen pickup from moisture in the air causes underbead cracking in steels that
harden as they cool from welding. To prevent such cracking, the steel is usually preheated
before welding. This retards the cooling rate of the weld and avoids martensite formation.
Postweld heat treatment, or stress relief, is also applied to some steels or for certain appli-
cations. The martensitic stainless steels behave in this fashion and, because of their high
hardenability, are quite difﬁcult to weld.
Austenitic stainless and nickel alloys do not harden, no matter how fast they cool from
welding. So, it is not necessary to preheat austenitic stainless, or to postweld heat treat.
Indeed preheating austenitic alloys beyond what may be necessary to dry the metal can be
harmful. Stress relief at 1100–1200ЊF (600–650ЊC) as applied to carbon steel is ineffective
with stainless or nickel alloys and may damage the corrosion resistance of some grades.
Stainless steel weldments are usually quite resistant to cracking, unless contaminated,
possibly by zinc or copper, more rarely by aluminum. A small amount of ferrite in the
austenitic weld bead provides this hot-cracking resistance.
10 Welding 55
High-nickel alloys are less forgiving and may be susceptible to cracking in restrained
joints, including heavy sections. This is a hot tearing, not a cold crack. That is, the weld
bead tears rather than stretches as the bead contracts upon solidifying.
This hot tearing/hot cracking has nothing to do with hardness. The faster a nickel alloy
weld freezes solid, the less time it spends in the temperature range where it can tear. For
this reason preheating, which slows down the cooling rate, is actually harmful, as it permits
more opportunity for hot tearing to occur.
4. Distortion. Stainless steel has poor thermal conductivity, only about one-fourth that
of ASTM A 36 structural steel. This means the welding heat tends to remain concentrated,
rather than spread out. Stainless steel also expands with heat about half again as much as
does carbon steel. The combination of these two factors means that stainless or nickel alloy
fabrications distort signiﬁcantly more than similar designs in carbon steel.
Tack welds should be closer than with carbon steel and sequenced in a pattern, left side,
right side, middle, etc. If the tacks are simply done in order from one end, the plate edges
close up. In order to balance stresses, weld runs should be done symmetrically about the
joint’s center of gravity. Back step welding is helpful. This subject is well covered in Refs.
10 and 11.
Reducing heat input reduces the stresses and distortions from the welding operation.
Heat into the workpiece is controlled by welding current, arc voltage, travel speed, and the
speciﬁc welding process used. For the same amperes, volts, and speed, submerged arc weld-
ing (SAW) transfers the most heat; shielded-metal arc welding (SMAW) and GMAW with
argon shielding next and roughly equivalent. Gas–tungsten arc welding (GTAW) can put the
least heat into the work.
5. Penetration. There is some tendency for welders to want to increase heat input with
the stainless and high-nickel alloys. First, the weld ﬁllers tend to be sluggish and not ﬂow
well, as compared with carbon steel. Second, the arc simply will not penetrate stainless steel
as it does carbon steel. The higher the nickel content, the less the penetration. Increasing
welding current will not solve the problem! Stainless, and especially nickel, alloy joint
designs must be more open. The base metal should be single or double beveled, with a root
gap, so that the weld metal may be placed in the joint.
6. Fabrication Time. Cleanliness, distortion control measures, maintaining low interpass
temperatures, and even machining add up to more time spent fabricating stainless than carbon
steel. A shop experienced with stainless steel may require 1.6 times as long to complete the
same fabrication in stainless as in carbon steel. A good carbon steel shop encountering
stainless or nickel alloys for the ﬁrst time may easily spend twice as long, maybe even three
times as long, to do the stainless steel fabrication as it would for the same job in carbon
10.2 Austenitic Alloys
The fundamental problem to be overcome in welding austenitic nickel-bearing alloys is the
tendency of the weld to hot tear upon solidiﬁcation from the melt. This matter is readily
handled in stainless steels of up to about 15% or so nickel. In these stainless steel grades
the weld metal composition is adjusted, usually by slightly higher chromium and reduced
nickel, to form a small amount of ferrite upon solidiﬁcation. The amount of ferrite in the
weld may be measured magnetically and is reported as a ferrite number (FN). This ferrite
acts to nullify the effects of the elements responsible for hot cracking in the Ni–Cr–Fe
austenitics. These elements are chieﬂy phosphorus, sulfur, silicon, and boron. In higher nickel
grades, about 20% nickel and over, it is metallurgically not possible to form any measurable
56 Stainless Steels
amount of ferrite. Therefore other means of minimizing hot cracking must be used. Foremost
among these is to use high-purity raw materials in the manufacture of weld ﬁllers. Simply
reducing the amounts of harmful P, S, Si, and B in the weld metal improves its ability to
make a sound weld. Phosphorus, in particular, must be kept below 0.015% in the weld wire
itself. Certain alloy additions such as manganese, columbium (niobium), and molybdenum
serve in one way or another to reduce the austenitic propensity for weld hot cracking.
Manganese ranges from about 2% in AWS E310-15 covered electrodes to 8% in ENiCrFe-
3 nickel alloy covered electrodes. Columbium at the 0.5% level, as in 347 or 20Cb-3 stainless
steel, is harmful whereas 2–4% Cb is quite beneﬁcial in many nickel-base weld ﬁllers.
Molybdenum is not added with the intention of increasing weldability; nevertheless it does
so. The 2% Mo contributes to 316L being the most weldable of the stainless steels, and 15%
in C-276 accounts for the popularity of the various ‘‘C-type’’ electrodes in repair welding.
The distinction between the lower nickel stainless steel grades, which depend upon
ferrite to ensure weldability, and the high-chnickel alloys, which require high-purity weld
ﬁllers, is an important one to remember. Most ferrite-containing (stainless) weld ﬁllers are
useless with nickel alloy base metal, as dilution of the weld bead with nickel from the base
metal eliminates this ferrite. Likewise a high-purity nickel alloy weld ﬁller, such as
ER320LR, may not be so crack resistant when contaminated by phosphorus from use on
316L or carbon steel base metal.
Alloys under 20% Nickel
Most austenitic grades containing less than 20% nickel are joined with weld ﬁllers that utilize
some ferrite, perhaps 4-12 FN, to ensure freedom from hot cracks. In practice, this means
stainless steels up through 317LMN or 309S, both about 13% nickel. The 310S type stands
in an odd position between the stainless and the nickel alloys, having neither ferrite nor
any particular alloy addition to the weld metal to ensure sound welds. Not surprisingly,
310S welds have a reputation for ﬁssuring, unless the ER310 weld ﬁller contains less than
Alloys over 20% Nickel
Corrosion-resistant alloys in this category begin with the 18% nickel 254 SMO᭨
, for this
and other ‘‘6 moly’’ grades are welded with an overmatching nickel alloy ﬁller such as
Other nickel alloys are joined with matching composition weld ﬁllers modiﬁed only by
restrictions on P, S, Si, and B. A minor amount of titanium may be added for deoxidation.
Other ﬁllers contain signiﬁcant manganese or columbium to improve resistance to ﬁssuring
and hot cracking.
Such chemistry modiﬁcations are rarely as effective as is the use of ferrite in the lower
nickel stainless weld ﬁllers. Welding technique and attention to cleanliness, then, become
increasingly important to ensure the soundness of fully austenitic welds. These techniques
include bead contour and low interpass temperature. Reinforced, convex stringer beads are
much more resistant to centerbead cracking than are shallow, concave beads. Interpass tem-
perature for most nickel alloy weldments is kept below 300ЊF (150ЊC). Cleanliness includes
not using oxygen additions to the GMAW shielding gases for nickel alloys.
It is worth repeating here that high-nickel alloys cannot be reliably welded using stain-
less steel weld ﬁllers. Stainless steel ﬁllers (308, 309, etc.) depend upon a chemistry which
will solidify from the melt as a duplex structure, containing a small amount of ferrite in
with the austenite.
10 Welding 57
10.3 Duplex Stainless Steels12
When welding duplex stainless steel, the issues are maintaining the austenite–ferrite balance
in the weldment and avoiding precipitation of nitrides and sigma. High heat input is used to
weld duplex, similar to welding 316L stainless steel. This is in contrast to the lower heat
preferred with the high-nickel alloys. Low heat input is not desirable with a duplex, as it
may not permit sufﬁcient transformation of ferrite to austenite upon cooling. Modern duplex
weld ﬁllers have a nitrogen addition as well as slightly higher nickel content than the base
metal. This is to ensure that enough weld metal ferrite transforms to austenite to maintain a
balance of the two phases.
Toughness and critical pitting temperature of duplex weldments vary with the choice of
welding process in opposite directions—in order of increasing notch impact toughness,
SMAW AC/DC, FCAW (ﬂux-cored arc welding), SMAW DC-basic, SAW, GMAW argon
shielding, GMAW 95% Ar–3% He–2% N2 shielding, and GTAW; in order of increasing
pitting resistance, as measured by critical pitting temperature, GTAW, GMAW, SAW, FCAW,
SMAW DC-basic, and SMAW AC/DC.
10.4 High-Molybdenum Alloys13
High-molybdenum stainless and nickel alloys are welded with an overmatching ﬁller metal.
This is necessary to maintain corrosion resistance in the weld metal at least equal to the
base metal. The reason is that molybdenum and chromium segregate as the weld metal
solidiﬁes from the melt. This leaves local areas with high and low molybdenum content.
Pitting corrosion can start in the low-Mo areas, with the pits eventually growing even into
metal with high molybdenum content. This occurs in alloys ranging from 316L to C-276,
for the most part being more severe at higher alloy contents
This matter began to receive attention when the 6% Mo stainless steels came on the
market. If any of these 6% Mo grades are welded without ﬁller metal, the result is a weld
bead that may be as low as 3% Mo in areas. The end result can be that this weld has only
the pitting corrosion resistance of 317L stainless. In the case of tubular products autogenously
welded in production, a high-temperature anneal is used to homogenize the metal. In addi-
tion, a small amount of nitrogen, 3–5%, is added to the torch gas. Fabrications of thin sheet,
which cannot be annealed after welding, should have this nitrogen addition to minimize the
loss of corrosion. Even so, because thin-sheet welds solidify more quickly, the segregation
is less severe.
In normal fabrication of a 6% Mo grade, alloy 625 (ERNiCrMo-3) ﬁller metal is used.
The weld metal contains 9% Mo. After welding, segregation causes some areas to have as
little as 6% Mo. The result is that the alloy 625 weld bead has approximately the same
corrosion resistance as the 6% Mo base metal. Higher alloy weld ﬁllers, such as ERNiCrMo-
10 or ERNiCrMo-14, may also be used, though the beneﬁt may be more theoretical than
real. ERNiCrMo-4 is not suggested, as it has 5% less chromium than does AL-6XN, for
example. Since the mid-1980s nearly all of the 6% Mo alloy fabrications have been made,
and put into service, using a 9% Mo weld ﬁller.
ERNiCrMo-3 weld ﬁller is widely available and is appropriate for welding lower alloys
such as 317L, 317LMN, and 904L for chloride service. The problem of reduced weld bead
corrosion resistance from molybdenum and chromium segregation exists with most of the
13–16% Mo nickel alloys as well. Filler 686 CPT (ERNiCrMo-14) does appear to be mark-
edly less susceptible to this effect than other high-molybdenum alloys.
58 Stainless Steels
Detailed technical information on heat and corrosion resistant alloys is available at
www.rolledalloys.com. Complete stainless steel data is at www.alleghenyludlum.com. Nickel
alloys in general are covered at www.nidi.org.
1. H. H. Uhlig, Corrosion Handbook, Wiley, New York, 1948
2. J. Kelly, Corrosion Resistant Alloy Speciﬁcations & Operating Data, Bulletin 151, Rolled Alloys,
Temperance, MI, 2003.
3. M. Ueda, H. Abo, T. Sunami, T. Muta, and H. Yamamoto, ‘‘A New Austenitic Stainless Steel Having
Resistance to Stress Corrosion Cracking,’’ Technical Report, Overseas No. 2, Nippon Steel, Tokyo,
January, 1973, p. 66.
4. C. H. Samans, ‘‘Stress Corrosion Cracking Susceptibility of Stainless Steels and Nickel Base Alloys
in Polythionic Acids and Acid Copper Sulfate Solution,’’ Corrosion 20, NACE International, Hous-
ton, TX, 1964.
5. J. Kelly, AL-6XN᭨
Alloy Physical, Mechanical and Corrosion Properties, Bulletin No. 210, Rolled
Alloys, Temperance, MI, 2002.
6. R. Kirchheiner, H. Portisch, R. Solomon, M. Jahudka, and J. Ettere, Designing Components for
Radioactive Waste Liquids in a Modern NiCrMo-Alloy, Paper No. 166, Corrosion 98, NACE Inter-
national, Houston, TX, 1998.
7. Paper No. 338, Corrosion 95, NACE International, Houston, TX, 1995.
8. Special Metals Publication No. SMC-092, Huntington, WV.
9. J. Kelly, Heat Resistant Alloy Welding, Bulletin No. 200, Rolled Alloys, Temperance, MI, 2002.
10. Avesta, Handbook for the Welding of Stainless Steel, Inf. 8901, Avesta Welding AB, Avesta, Sweden.
11. B. Lundqvist, The Sandvik Welding Handbook, AB Sandvik Steel, Sandviken, Sweden, 1977.
12. J. Kelly, RA2205 Duplex Stainless, Bulletin No. 1071, Rolled Alloys, Temperance, MI, 2003.
13. J. Kelly, AL-6XN Alloy Fabrication, Bulletin No. 203, Rolled Alloys, Temperance, MI, 2001.
RA333 and RA330 are registered trademarks of Rolled Alloys, Inc.
AL-6XN, AL 2003, E-BRITE, and AL 29-4C are registered trademarks, and 317LXN a trademark, of
ATI Properties, Inc.
7MoPLUS and 20Cb-3 are registered trademarks of Carpenter Technology Corporation.
254 SMO and 654 SMO are registered trademarks of Outokumpu AB.
Nicrofer is a registered trademark of ThyssenKrupp VDM.
Duriron is a registered trademark of Duraloy Technologies, Inc.
Hastelloy, Haynes, G-30, and C-2000 are registered trademarks, and D-205 a trademark, of Haynes
Incoloy, Inconel, Monel, 800HT, 25-6MO, and 27-7MO are registered trademarks of Special Metals,
Nintronic, 17-4PH, PH15-7MO, 17-7PH, and PH13-8MO are registered trademarks of AK Steel Cor-
Oakite is a registered trademark of Oakite Products, Inc.
Sandvik SX and SAF are registered trademarks of Sandvik AB.
J. G. Kaufman
1 NATURE OF ALUMINUM
2 ADVANTAGES OF
ALUMINUM ALLOYS 60
Aluminum Alloys 60
2.2 Cast Aluminum Alloys 62
2.3 Limitations of Wrought and
Cast Aluminum Alloys 62
3 DESIGNATION SYSTEMS 63
3.1 Wrought Aluminum Alloy
Designation System 64
3.2 Cast Aluminum Alloy
Designation System 65
3.3 Aluminum Alloy Temper
Designation System 68
4 MECHANICAL PROPERTIES OF
ALUMINUM ALLOYS 71
5 CORROSION BEHAVIOR OF
ALUMINUM ALLOYS 86
5.1 General Corrosion 86
5.2 Pitting Corrosion 87
5.3 Galvanic Corrosion 87
6 MACHINING ALUMINUM
6.1 Single-Point Tool Operations 88
6.2 Multipoint Tool Operations 88
7 FINISHING ALUMINUM 90
7.1 Mechanical Finishes 90
7.2 Chemical Finishes 90
7.3 Electrochemical Finishes 90
7.4 Clear Anodizing 91
7.5 Color Anodizing 91
7.6 Integral Color Anodizing 91
7.7 Electrolytically Deposited
7.8 Hard Anodizing 91
7.9 Electroplating 91
7.10 Applied Coatings 91
8 APPLICATIONS OF ALUMINUM
8.1 Applications by Alloy Class 92
8.2 Applications by Market Area 111
9 SUMMARY 114
1 NATURE OF ALUMINUM ALLOYS
Aluminum is the most abundant metal and the third most abundant chemical element in the
earth’s crust, comprising over 8% of its weight. Only oxygen and silicon are more prevalent.
Yet, until about 150 years ago aluminum in its metallic form was unknown to humans. The
reason for this is that aluminum, unlike iron or copper, does not exist as a metal in nature.
Because of its chemical activity and its afﬁnity for oxygen, aluminum is always found
combined with other elements, mainly as aluminum oxide. As such it is found in nearly all
clays and many minerals. Rubies and sapphires are aluminum oxide colored by trace im-
purities, and corundum, also aluminum oxide, is the second hardest naturally occurring sub-
stance on earth—only a diamond is harder. It was not until 1886 that scientists learned how
to economically extract aluminum from aluminum oxide via electrolytic reduction. Yet in
the more than 100 years since that time, aluminum has become the second most widely used
of the approximately 60 naturally occurring metals, second only to iron.
Aluminum alloys are broadly used in products and applications that touch us regularly
in our daily lives, from aluminum foil for food packaging and easy-open aluminum cans for
Mechanical Engineers’ Handbook: Materials and Mechanical Design, Volume 1, Third Edition.
Edited by Myer Kutz
Copyright 2006 by John Wiley & Sons, Inc.
60 Aluminum Alloys
your beverages to the structural members of the aircraft in which we travel. The broad use
of aluminum alloys is dictated by a very desirable combination of properties, combined with
the ease with which they may be produced in a great variety of forms and shapes. In this
chapter, we will review the characteristics of aluminum alloys that make them so attractive
and note the variety of applications in which they are used.
For readers who are interested in a broader look at the aluminum industry as a whole,
the publications of the Aluminum Association are highly recommended, especially:
• Aluminum: Technology, Applications, and Environment1
• Aluminum Standards and Data (Standard and Metric Editions)2
• Standards for Aluminum Sand and Permanent Mold Castings3
• The Aluminum Design Manual4
See the References at the end of the chapter for a more complete listing.
2 ADVANTAGES OF ALUMINUM ALLOYS
The ﬁrst step in becoming familiar with the opportunities to utilize aluminum alloys advan-
tageously is to brieﬂy note some of the basic characteristics of wrought and cast aluminum
alloys that make them desirable candidates for such a wide range of applications as well as
their limitations. Wrought alloys (those mechanically formed by rolling, forging, and extru-
sion into useful products) are addressed ﬁrst, then cast alloys (those cast directly to the near-
ﬁnal ﬁnished shape).
2.1 Wrought Aluminum Alloys
Low Density/Speciﬁc Gravity. One property of aluminum that everyone is familiar with is
its light weight or, technically, its low density or speciﬁc gravity. The speciﬁc gravity of
aluminum is only 2.7 times that of water and roughly one-third that of steel and copper. An
easy number to remember is that 1 cubic inch (in.3
) of aluminum weighs 0.1 lb; 1 cubic
) weighs 170 lb compared to 62 lb for water and 490 lb for steel.
High Strength–Weight Ratio. The combination of relatively high strength with low density
means a high strength efﬁciency for aluminum alloys and many opportunities for replacement
of heavier metals with no loss (and perhaps a gain) in load-carrying capacity. This charac-
teristic, combined with the excellent corrosion resistance and recyclability, has led to alu-
minum’s broad use in containers, aircraft, and automotive applications.
Excellent Corrosion Resistance. As a result of a naturally occurring tenacious surface oxide
ﬁlm, many aluminum alloys provide exceptionally resistance to corrosion in many atmos-
phere and chemical environments. Alloys of the 1xxx, 3xxx, 5xxx, and 6xxx systems are
especially favorable in this respect and are even used in applications where they are in direct
contact with seawater and antiskid salts. With some electrocoating enhancements (e.g., an-
odizing), the oxide coating can be thickened for even greater protection. Aluminum and a
number of its alloys possess excellent resistance to corrosive attack by many foods and
chemicals as well as natural environments.
High Thermal Conductivity. Aluminum and its alloys are good conductors of heat, and, while
they melt at lower temperatures than steels, about 1000ЊF (about 535ЊC), they are slower to
reach very high temperatures than steel in ﬁre exposure.
2 Advantages of Aluminum Alloys 61
High Electrical Conductivity. Pure aluminum and some of its alloys have exceptionally high
electrical conductivity (i.e., very low electrical resistivity), second only to copper among
common metals as conductors.
Excellent Reﬂectivity. Aluminum with appropriate surface treatment becomes an excellent
reﬂector and does not dull from normal atmospheric oxidation.
High Fracture Toughness and Energy Absorption Capacity. Many aluminum alloys are ex-
ceptionally tough and excellent choices for critical applications where resistance to unstable
crack growth and brittle fracture are imperatives. Alloys of the 5xxx series, for example, are
prime choices for liqueﬁed natural gas (LNG) tankage. And special high-toughness versions
of aerospace alloys, such as 2124, 7050, and 7475, replace the standard versions of these
alloys for critical bulkhead applications.
Superior Cryogenic Toughness. Aluminum alloys, especially of the 3xxx, 5xxx, and 6xxx
series, are ideal for very low temperature applications because the ductility and toughness
as well as strength of many alloys at subzero temperatures are as high as or higher than at
room temperature, even down to near absolute zero. As noted above, the 5xxx series alloys
are regularly used for liqueﬁed gas tankage operating at temperatures from Ϫ150 to Ϫ452ЊF
(Ϫ65 to Ϫ269ЊC)
Fatigue Strength. On an efﬁciency basis (strength to density) the fatigue strengths of many
aluminum alloys are comparable to those of steels.
Low Modulus of Elasticity. Aluminum alloys have elastic moduli about one-third those of
steels (about 10 ϫ 106
psi vs. about 30 ϫ 106
psi), so they absorb about three times as much
elastic energy upon deformation to the same stress. They also deﬂect three times more under
load (see Section 2.3).
Superior Workability. Aluminum alloys are readily workable by virtually all metalworking
technologies and especially amenable to extrusion (the process of forcing heated metal
through shaped dies to produce speciﬁc shaped sections). This enables aluminum to be
produced in a remarkable variety of shapes and forms in which the metal can be placed in
locations where it can most efﬁciently carry the applied loads.
Ease of Joining. Aluminum alloys may be joined by a very broad variety of commercial
methods, including welding, brazing, soldering, riveting, bolting, and even nailing in addition
to an unlimited variety of mechanical procedures. Welding, while considered difﬁcult by
those familiar only with joining steel and who try to apply the same techniques to aluminum,
is particularly easy when performed by proven techniques such as gas–metal arc welding
(GMAW or MIG) or gas–tungsten arc welding (GTAW or TIG).
Versatile Array of Finishes. Aluminum can be ﬁnished in more ways than any other metal
used today, including a variety of techniques that build upon its strong oxide coating and
employ coloring, plus more conventional means such as painting and enameling.
Ease of Recyclability. Aluminum and its alloys are among the easiest to recycle of any
structural materials. And they are recyclable in the truest sense, unlike materials which are
reused but in lower quality products: Aluminum alloys may be recycled directly back into
the same high-quality products like rigid container sheet (cans) and automotive components.
Through such recycling, the life-cycle assessment advantages for aluminum are optimized.
62 Aluminum Alloys
2.2 Cast Aluminum Alloys
The desirable characteristics of wrought alloys are also generally applicable to cast alloys,
but in fact the choice of one casting alloy or another tends to be more often made on the
basis of their relative abilities to meet one or more of the four following characteristics:
• Ease of casting
• Quality of ﬁnish
• High strength, especially at high temperatures
• High toughness
1. Ease of Casting. Many aluminum casting alloys have relatively high silicon contents
that provide excellent ﬂow characteristics during casting, enabling them to be utilized for
large and complex castings (e.g., even complete engines). Relatively minute details in the
shape of the casting can be accurately and reliably replicated.
2. Quality of Finish. By proper selection of aluminum casting alloy, extremely ﬁne
surface quality can be achieved. While such alloys typically require more attention to casting
practice, they are widely used in applications where the ﬁnished casting surface mirrors the
ﬁnish needed in surface.
3. High Strength. Many aluminum casting alloys respond to heat treatment following
casting and achieve relatively high levels of strength and excellent strength–weight ratios.
With careful design of molds, high chill rates can be assured and both high strength and
high toughness can be achieved.
4. High Toughness. With careful selection of alloy and heart treatment combined with
process technology often referred to as premium engineered casting, optimizing metal ﬂow
and chill rated, the toughness of castings may be comparable to that of wrought alloys at
comparable strength levels. Techniques such as hot isostatic pressing (HIP) are available to
further reduce porosity and improve performance.
Unfortunately few casting alloys possess all four characteristics, but some generaliza-
tions useful in alloy selection for speciﬁc applications may be made:
1. Ease of Casting. The high-silicon 3xx.x series are outstanding in this respect as the
relatively high silicon contents lend a characteristic of good ﬂow and mold-ﬁlling capability.
As a result, the 3xxx.x series are the most widely used and are especially chosen for large
and very complex casting.
2. Finish. The 5xx.x and 7xx.x series are noteworthy for the ﬁne ﬁnish they provide,
but they are more difﬁcult to cast than the 3xx.x series and so are usually limited to those
applications where that ﬁnish is paramount. A good example is the use of 7xx.x alloys for
3. Strength and Toughness. The 2xx.x alloys typically provide the very highest
strengths, especially at high temperatures, but are among the more difﬁcult to cast and lack
good surface characteristics. Therefore their use is usually limited to situations where so-
phisticated casting techniques can be applied and where strength and toughness are at a
premium, as in the aerospace industry. Relatively high strengths and superior toughness can
also be achieved with some of the higher purity 3xx.x alloys (e.g., A356.0, A357.0) in heat-
2.3 Limitations of Wrought and Cast Aluminum Alloys
There are several characteristics of aluminum alloys that require special attention in alloy
selection or design:
3 Designation Systems 63
Moduli of Elasticity. As noted earlier, the elastic moduli of aluminum alloys are about one-
third those of steel. In applications such as bridges, where some designs may be deﬂection
critical, this is a disadvantage and consideration should be given to the fact that aluminum
alloys will deﬂect about three times more than comparably sized steel members. To com-
pensate for this, aluminum members subject to bending loads are usually made deeper or
thicker in their upper and lower extremities to reduce stresses and/or deﬂections.
Melting Temperature. Aluminum Alloys melt at about 1000ЊF (535ЊC), well below where
steels melt, and so they should not be selected for applications such as ﬂue pipes and ﬁre
doors where the low melting point may result in unsatisfactory performance. The useful limit
of high-temperature structural application of aluminum alloys is about 500ЊF (about 260ЊC)
for conventional alloys or about 600ЊF (315ЊC) for alumina-enhanced alloys. It is useful to
note, however, that even in the most intense ﬁres, aluminum alloys do not burn; they are
rated noncombustible in all types of ﬁre tests and achieve the highest ratings in ﬂame-spread
tests. Further, as noted earlier, they are slower to reach high temperatures in ﬁres than other
metals such as steels because of their higher thermal conductivity and emmissivity. Never-
theless, they should not be used where service requirements include structural strength above
500ЊF (260ЊC) or exposure above 700ЊF (370ЊC).
Stress–Corrosion Susceptibility of Some Alloys. Some aluminum alloys, notably the 2xxx
and 7xxx alloys, when stressed perpendicular to the major plane of grain ﬂow (i.e., in the
short-transverse direction) may be subject to intergranular stress–corrosion cracking (SCC)
unless they have been given a special thermal treatment to reduce or eliminate this type of
behavior. If short transverse stresses are anticipated in relatively thick components, 2xxx
alloys should only be utilized in the T6- or T8-type tempers (not T3- or T4-type tempers),
and 7xxx alloys should only be used in the T7-type tempers (not T6- or T8-type tempers).
Similarly, 5xxx alloys with more than 3% Mg should not be used in applications where a
combination of high stress and high temperature will be experienced over a long period of
time (more than several hundred hours at or above 150ЊF, or 65ЊC) because some suscepti-
bility to SCC may be encountered (i.e., the alloys may become ‘‘sensitized’’); for applications
where temperatures above about 150ЊF (65ЊC) are likely to be encountered for long periods,
the use of 5xxx alloys with 3% or less Mg, e.g., 5454, is recommended.
Mercury Embrittlement. Aluminum alloys should never be used when they may be in direct
contact with liquid or vaporized mercury; severe grain-boundary embrittlement may result.
This is an unlikely exposure for the vast majority of applications, but in any instance where
there is the possibility of mercury being present, the use of aluminum alloys should be
3 DESIGNATION SYSTEMS
One advantage in using aluminum alloys and tempers is the universally accepted and easily
understood alloy and temper systems by which they are known. It is extremely useful for
both secondary fabricators and users of aluminum products and components to have a work-
ing knowledge of those designation systems. The alloy system provides a standard form of
alloy identiﬁcation that enables the user to understand a great deal about the chemical com-
position and characteristics of the alloy, and similarly, the temper designation system permits
one to understand a great deal about the way in which the product has been fabricated.
The alloy and temper designation systems in use today for wrought aluminum were
adopted by the aluminum industry in about 1955, and the current system for cast system
64 Aluminum Alloys
Table 1 Main Alloying Elements in Wrought Alloy
Alloy Main Alloying Element
1000 Mostly pure aluminum; no major alloying additions
6000 Magnesium and silicon
8000 Other elements (e.g., iron or tin)
was developed somewhat later. The aluminum industry managed the creation and continues
the maintenance of the systems through its industry organization, the Aluminum Association.
The alloy registration process is carefully controlled and its integrity maintained by the
Technical Committee on Product Standards of the Aluminum Association, made up of in-
dustry standards experts.5
Further, as noted earlier, the Aluminum Association designation
system is the basis of the American National Standards Institute (ANSI) standards, incor-
porated in ANSI H35.16
and, for the wrought alloy system at least, is the basis of the near-
worldwide International Accord on Alloy Designations.7
It is useful to note that the
international accord does not encompass casting alloy designations, so more variation will
be encountered in international designations for casting alloys than for wrought aluminum
The Aluminum Association Alloy and Temper Designation Systems covered in ANSI
and Aluminum Standards and Data2
are outlined in this chapter.
3.1 Wrought Aluminum Alloy Designation System
The Aluminum Association Wrought Alloy Designation System consists of four numerical
digits, sometimes with alphabetic preﬁxes or sufﬁces, but normally just the four numbers:
• The ﬁrst digit deﬁnes the major alloying class of the series starting with that number.
• The second deﬁnes variations in the original basic alloy; that digit is always a 0 for
the original composition, a 1 for the ﬁrst variation, a 2 for the second variation, and
so forth; variations are typically deﬁned by differences in one or more alloying ele-
ments of 0.15–0.50% or more, depending upon the level of the added element.
• The third and fourth digits designate the speciﬁc alloy within the series; there is no
special signiﬁcance to the values of those digits, and they are not necessarily used in
Table 1 shows the meaning of the ﬁrst of the four digits in the wrought alloy designation
system. The alloy family is identiﬁed by that number and the associated main alloying
ingredient(s), with three exceptions:
• Members of the 1000 series family are commercially pure aluminum or special-purity
versions and as such do not typically have any alloying elements intentionally added;
however they do contain minor impurities that are not removed unless the intended
application requires it.
3 Designation Systems 65
• The 8000 series family is an ‘‘other elements’’ series, comprised of alloys with rather
unusual major alloying elements such as iron and nickel.
• The 9000 series is unassigned.
The major beneﬁt of understanding this designation system is that one can tell a great
deal about the alloy just from knowledge of which it is a member. For example:
• As indicated earlier, the 1xxx series are pure aluminum and its variations; composi-
tions of 99.0% or more aluminum are by deﬁnition in this series. Within the 1xxx
series, the last two of the four digits in the designation indicate the minimum alumi-
num percentage. These digits are the same as the two digits to the right of the decimal
point in the minimum aluminum percentage speciﬁed for the designation when ex-
pressed to the nearest 0.01%. As with the rest of the alloy series, the second digit
indicates modiﬁcations in impurity limits or intentionally added elements. Composi-
tions of the 1xxx series do not respond to any solution heat treatment but may be
strengthened modestly by strain hardening.
• The 2xxx series alloys have copper as their main alloying element and, because it
will go in signiﬁcant amounts into solid solution in aluminum, they will respond to
solution heat treatment; they are referred to as heat treatable.
• The 3xxx series alloys are based on manganese and are strain hardenable; they do not
respond to solution heat treatment.
• The 4xxx series alloys are based on silicon; some alloys are heat treatable, others are
not, depending upon the amount of silicon and the other alloying constituents.
• The 5xxx series alloys are based on magnesium and are strain hardenable, not heat
• The 6xxx series alloys have both magnesium and silicon as their main alloying ele-
ments; these combine as magnesium silicide (Mg2Si) following solid solution, and so
the alloys are heat treatable.
• The 7xxx series alloys have zinc as their main alloying element, often with signiﬁcant
amounts of copper and magnesium, and they are heat treatable.
• The 8xxx series contain one or more of several less frequently used major alloying
elements like iron or tin; their characteristics depend on the major alloying element(s).
The compositions of a representative group of widely used commercial wrought alu-
minum alloys are given in Table 2, from Aluminum Standards and Data2
and other Alumi-
num Association publications.
3.2 Cast Aluminum Alloy Designation System
The designation system for cast aluminum alloys is similar in some respects to that for
wrought alloys but has a few very important differences as noted by the following descrip-
Like the wrought alloy system, the cast alloy designation system also has four digits
but differs from the wrought alloy system in that a decimal point is used between the third
and fourth digits to make clear that these are designations to identify alloys in the form of
castings or foundry ingot.
As for the wrought alloy designation system, the various digits of the cast alloy system
convey information about the alloy: